 
data_56-2
 
_audit_creation_method            'SHELXL-2018/3'
_shelx_SHELXL_version_number      '2018/3'
_chemical_name_systematic         ?
_chemical_name_common             ?
_chemical_melting_point           ?
_chemical_formula_moiety          ?
_chemical_formula_sum
 'Al2.39 H2 Ca0.94 Ce3.07 Fe1.06 Mg0.38 Mn0.16 O22 Si5' 
_chemical_formula_weight          1103.53

loop_
 _atom_type_symbol
 _atom_type_description
 _atom_type_scat_dispersion_real
 _atom_type_scat_dispersion_imag
 _atom_type_scat_source
 'O'  'O'   0.0106   0.0060
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mg'  'Mg'   0.0486   0.0363
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Al'  'Al'   0.0645   0.0514
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Si'  'Si'   0.0817   0.0704
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ca'  'Ca'   0.2262   0.3064
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Mn'  'Mn'   0.3368   0.7283
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Fe'  'Fe'   0.3463   0.8444
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'Ce'  'Ce'  -0.2486   2.6331
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 'H'  'H'   0.0000   0.0000
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
 
_space_group_crystal_system       monoclinic
_space_group_IT_number            11
_space_group_name_H-M_alt         'P 21/m'
_space_group_name_Hall            '-P 2yb'
 
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
 
loop_
 _space_group_symop_operation_xyz
 'x, y, z'
 '-x, y+1/2, -z'
 '-x, -y, -z'
 'x, -y-1/2, z'
 
_cell_length_a                    8.9652(4)
_cell_length_b                    5.7306(2)
_cell_length_c                    17.6770(9)
_cell_angle_alpha                 90
_cell_angle_beta                  116.053(6)
_cell_angle_gamma                 90
_cell_volume                      815.88(7)
_cell_formula_units_Z             2
_cell_measurement_temperature     293(2)
_cell_measurement_reflns_used     2959
_cell_measurement_theta_min       3.2970
_cell_measurement_theta_max       30.8070
 
_exptl_crystal_description        'irreguar'
_exptl_crystal_colour             'black'
_exptl_crystal_density_meas       ?
_exptl_crystal_density_method     ?
_exptl_crystal_density_diffrn     4.492          
_exptl_crystal_F_000              1024
_exptl_transmission_factor_min    ?
_exptl_transmission_factor_max    ?
_exptl_crystal_size_max           0.0710
_exptl_crystal_size_mid           0.0485
_exptl_crystal_size_min           0.0324
_exptl_absorpt_coefficient_mu     10.370
_shelx_estimated_absorpt_T_min    ?
_shelx_estimated_absorpt_T_max    ?
_exptl_absorpt_correction_type    'gaussian'
_exptl_absorpt_correction_T_min   0.658
_exptl_absorpt_correction_T_max   0.804
_exptl_absorpt_process_details    
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.34 (release 22-05-2014 CrysAlis171 .NET)
(compiled May 22 2014,16:03:01)
Numerical absorption correction based on gaussian integration over
			a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_absorpt_special_details    ?
_diffrn_ambient_temperature       293(2)
_diffrn_radiation_wavelength      0.71073
_diffrn_radiation_type            MoK\a
_diffrn_source                    'Enhance (Mo) X-ray Source'
_diffrn_measurement_device_type   'Xcalibur, Sapphire3'
_diffrn_measurement_method        'ω scans'
_diffrn_detector_area_resol_mean  16.0630
_diffrn_reflns_number             14151
_diffrn_reflns_av_unetI/netI      0.0473
_diffrn_reflns_av_R_equivalents   0.0710
_diffrn_reflns_limit_h_min        -11
_diffrn_reflns_limit_h_max        11
_diffrn_reflns_limit_k_min        -7
_diffrn_reflns_limit_k_max        7
_diffrn_reflns_limit_l_min        -23
_diffrn_reflns_limit_l_max        23
_diffrn_reflns_theta_min          3.301
_diffrn_reflns_theta_max          28.282
_diffrn_reflns_theta_full         25.242
_diffrn_measured_fraction_theta_max   0.998
_diffrn_measured_fraction_theta_full  0.997
_diffrn_reflns_Laue_measured_fraction_max    0.998
_diffrn_reflns_Laue_measured_fraction_full   0.997
_diffrn_reflns_point_group_measured_fraction_max   0.998
_diffrn_reflns_point_group_measured_fraction_full  0.997
_reflns_number_total              2218
_reflns_number_gt                 2040
_reflns_threshold_expression      'I > 2σ(I)'
_reflns_Friedel_coverage          0.000
_reflns_Friedel_fraction_max      .
_reflns_Friedel_fraction_full     .
 
_reflns_special_details
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
 
_computing_data_collection        ?
_computing_cell_refinement        ?
_computing_data_reduction         ?
_computing_structure_solution     ?
_computing_structure_refinement 'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_molecular_graphics     ?
_computing_publication_material   ?
_refine_special_details           ?
_refine_ls_structure_factor_coef  Fsqd
_refine_ls_matrix_type            full
_refine_ls_weighting_scheme       calc
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0240P)²+16.4905P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary      ?
_atom_sites_solution_secondary    ?
_atom_sites_solution_hydrogens    difmap
_refine_ls_hydrogen_treatment     refxyz
_refine_ls_extinction_method      none
_refine_ls_extinction_coef        .
_refine_ls_number_reflns          2218
_refine_ls_number_parameters      199
_refine_ls_number_restraints      2
_refine_ls_R_factor_all           0.0850
_refine_ls_R_factor_gt            0.0752
_refine_ls_wR_factor_ref          0.1218
_refine_ls_wR_factor_gt           0.1186
_refine_ls_goodness_of_fit_ref    1.384
_refine_ls_restrained_S_all       1.383
_refine_ls_shift/su_max           0.000
_refine_ls_shift/su_mean          0.000
 
loop_
 _atom_site_label
 _atom_site_type_symbol
 _atom_site_fract_x
 _atom_site_fract_y
 _atom_site_fract_z
 _atom_site_U_iso_or_equiv
 _atom_site_adp_type
 _atom_site_occupancy
 _atom_site_site_symmetry_order  
 _atom_site_calc_flag
 _atom_site_refinement_flags_posn
 _atom_site_refinement_flags_adp
 _atom_site_refinement_flags_occupancy
 _atom_site_disorder_assembly
 _atom_site_disorder_group
Ce Ce 0.7304(4) 0.250000 0.40892(19) 0.0197(11) Uani 0.067(7) 2 d S T P . .
Ca Ca 0.7304(4) 0.250000 0.40892(19) 0.0197(11) Uani 0.933(7) 2 d S T P . .
Ce2 Ce 0.89180(11) 0.250000 0.25072(5) 0.0147(2) Uani 1 2 d S T P . .
Ce3 Ce 0.73836(13) 0.250000 0.00931(6) 0.0314(3) Uani 1 2 d S T P . .
Ce4 Ce 0.07783(11) 0.750000 0.16589(6) 0.0140(2) Uani 1 2 d S T P . .
Fe1 Fe 0.500000 0.500000 0.500000 0.0111(7) Uani 0.34 2 d S . P . .
Al1 Al 0.500000 0.500000 0.500000 0.0111(7) Uani 0.52 2 d S . P . .
Mg1 Mg 0.500000 0.500000 0.500000 0.0111(7) Uani 0.14 2 d S . P . .
Fe2 Fe 0.4794(4) 0.0005(6) 0.20533(19) 0.0120(9) Uani 0.065(13) 1 d . . P . .
Al2 Al 0.4794(4) 0.0005(6) 0.20533(19) 0.0120(9) Uani 0.935(13) 1 d . . P . .
Fe3 Fe 0.1888(3) 0.750000 0.37674(16) 0.0149(6) Uani 0.6 2 d S T P . .
Mg3 Mg 0.1888(3) 0.750000 0.37674(16) 0.0149(6) Uani 0.24 2 d S T P . .
Mn3 Mn 0.1888(3) 0.750000 0.37674(16) 0.0149(6) Uani 0.16 2 d S T P . .
Si1 Si 0.1595(5) 0.250000 0.4790(2) 0.0079(8) Uani 1 2 d S T P . .
Si2 Si 0.8003(5) 0.750000 0.3351(3) 0.0094(8) Uani 1 2 d S T P . .
Si3 Si 0.3025(5) 0.250000 0.3118(2) 0.0085(8) Uani 1 2 d S T P . .
Si4 Si 0.6700(5) 0.750000 0.1037(3) 0.0126(8) Uani 1 2 d S T P . .
Si5 Si 0.1550(5) 0.250000 0.0782(3) 0.0091(8) Uani 1 2 d S T P . .
O1 O 0.2624(9) 0.4909(13) 0.4834(5) 0.0170(17) Uani 1 1 d . . . . .
O2 O 0.1784(9) 0.4742(14) 0.2901(5) 0.0153(16) Uani 1 1 d . . . . .
O3 O 0.6912(9) 0.9866(13) 0.2998(5) 0.0145(16) Uani 1 1 d . . . . .
O4 O 0.4382(13) 0.750000 0.4239(7) 0.017(2) Uani 1 2 d S T P . .
O5 O 0.4485(12) 0.250000 0.4109(6) 0.015(2) Uani 1 2 d S T P . .
O6 O 0.4142(12) 0.250000 0.2586(6) 0.012(2) Uani 1 2 d S T P . .
O7 O -0.0161(12) 0.250000 0.3978(6) 0.014(2) Uani 1 2 d S T P . .
O8 O 0.9490(14) 0.750000 0.3069(8) 0.025(3) Uani 1 2 d S T P . .
O9 O 0.8755(15) 0.750000 0.4371(7) 0.025(3) Uani 1 2 d S T P . .
O10 O 0.5577(13) 0.250000 0.1639(7) 0.014(2) Uiso 1 2 d DS . P . .
H1 H 0.512(19) 0.250000 0.1103(9) 0.016 Uiso 1 2 d DS U P . .
O11 O 0.4007(12) 0.750000 0.2471(6) 0.009(2) Uani 1 2 d DS T P . .
H2 H 0.415(19) 0.750000 0.298(3) 0.011 Uiso 1 2 d DS U P . .
O12 O 0.5388(11) 0.750000 0.1480(6) 0.010(2) Uani 1 2 d S T P . .
O13 O 0.2680(9) 0.4876(13) 0.1095(5) 0.0150(16) Uani 1 1 d . . . . .
O14 O 0.7930(10) -0.0272(14) 0.1321(5) 0.0191(17) Uani 1 1 d . . . . .
O15 O 0.5525(19) 0.684(3) 0.0055(9) 0.023(4) Uani 0.5 1 d . . P . .
O16 O 0.0628(18) 0.250000 -0.0218(8) 0.040(4) Uani 1 2 d S T P . .
O17 O 0.0241(14) 0.250000 0.1161(8) 0.028(3) Uani 1 2 d S T P . .
 
 
_geom_special_details
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
 
loop_
 _geom_bond_atom_site_label_1
 _geom_bond_atom_site_label_2
 _geom_bond_distance
 _geom_bond_site_symmetry_2
 _geom_bond_publ_flag
Ca O3 2.350(8) 1_545 ?
Ca O3 2.350(8) 4_575 ?
Ca O7 2.365(11) 1_655 ?
Ca O1 2.393(8) 3_666 ?
Ca O1 2.393(8) 2_646 ?
Ca O5 2.543(11) . ?
Ca O6 2.913(10) . ?
Ca O9 3.095(5) . ?
Ca O9 3.095(5) 1_545 ?
Ca Si2 3.320(3) . ?
Ca Si2 3.320(3) 1_545 ?
Ca Si1 3.375(3) 3_666 ?
Ce2 O7 2.357(10) 1_655 ?
Ce2 O14 2.465(8) . ?
Ce2 O14 2.465(8) 4_565 ?
Ce2 O2 2.677(8) 1_655 ?
Ce2 O2 2.677(8) 4_665 ?
Ce2 O10 2.700(10) . ?
Ce2 O3 2.763(8) 1_545 ?
Ce2 O3 2.763(8) 4_575 ?
Ce2 O8 3.002(4) 1_545 ?
Ce2 O8 3.002(4) . ?
Ce2 O17 3.090(13) 1_655 ?
Ce2 Si3 3.352(4) 1_655 ?
Ce2 Si2 3.490(2) 1_545 ?
Ce2 Si2 3.490(2) . ?
Ce2 Si1 3.680(4) 1_655 ?
Ce2 Fe2 3.708(3) . ?
Ce2 Fe2 3.708(3) 4_565 ?
Ce3 O17 2.425(11) 1_655 ?
Ce3 O15 2.532(16) 2_645 ?
Ce3 O15 2.532(16) 3_665 ?
Ce3 O14 2.557(8) 4_565 ?
Ce3 O14 2.557(8) . ?
Ce3 O13 2.563(8) 2_645 ?
Ce3 O13 2.563(8) 3_665 ?
Ce3 O12 2.800(10) 3_665 ?
Ce3 O15 2.977(16) 4_565 ?
Ce3 O15 2.977(16) . ?
Ce3 O16 3.188(15) 1_655 ?
Ce3 Si4 3.312(4) 3_665 ?
Ce3 O16 3.331(8) 3_665 ?
Ce3 O16 3.331(8) 3_655 ?
Ce3 Si5 3.383(4) 1_655 ?
Ce3 Si4 3.503(3) 1_545 ?
Ce3 Si4 3.503(3) . ?
Ce3 Si5 3.579(3) 3_655 ?
Ce3 Si5 3.579(3) 3_665 ?
Ce3 O15 3.635(15) 1_545 ?
Ce4 O16 2.293(12) 3_565 ?
Ce4 O2 2.528(7) . ?
Ce4 O2 2.528(7) 4_575 ?
Ce4 O11 2.605(10) . ?
Ce4 O14 2.677(8) 4_465 ?
Ce4 O14 2.677(8) 1_465 ?
Ce4 O13 2.767(8) . ?
Ce4 O13 2.767(8) 4_575 ?
Ce4 O17 2.974(3) 1_565 ?
Ce4 O17 2.974(3) . ?
Ce4 O8 3.174(11) 1_455 ?
Ce4 Si4 3.324(4) 1_455 ?
Ce4 Fe3 3.409(3) . ?
Ce4 Si5 3.469(2) . ?
Ce4 Si5 3.469(2) 1_565 ?
Ce4 Fe2 3.648(3) 1_565 ?
Ce4 Fe2 3.648(3) 4_565 ?
Ce4 Si3 3.789(3) 1_565 ?
Fe1 O4 1.875(7) . ?
Fe1 O4 1.875(7) 3_666 ?
Fe1 O1 2.019(7) 3_666 ?
Fe1 O1 2.019(7) . ?
Fe1 O5 2.027(7) 3_666 ?
Fe1 O5 2.027(7) . ?
Fe1 Fe1 2.86530(10) 2_656 ?
Fe1 Fe1 2.86530(10) 2_646 ?
Fe2 O10 1.878(8) . ?
Fe2 O11 1.888(7) 1_545 ?
Fe2 O3 1.902(8) 1_545 ?
Fe2 O13 1.909(8) 4_565 ?
Fe2 O6 1.938(8) . ?
Fe2 O12 1.961(8) 1_545 ?
Fe2 Fe2 2.860(7) 4_565 ?
Fe2 Fe2 2.871(7) 4 ?
Fe3 O8 1.953(12) 1_455 ?
Fe3 O4 2.014(11) . ?
Fe3 O2 2.174(8) 4_575 ?
Fe3 O2 2.174(8) . ?
Fe3 O1 2.258(8) 4_575 ?
Fe3 O1 2.258(8) . ?
Si1 O7 1.598(11) . ?
Si1 O1 1.644(8) . ?
Si1 O1 1.644(8) 4_565 ?
Si1 O9 1.644(12) 3_666 ?
Si2 O8 1.615(12) . ?
Si2 O9 1.624(11) . ?
Si2 O3 1.627(8) . ?
Si2 O3 1.627(8) 4_575 ?
Si3 O2 1.631(8) . ?
Si3 O2 1.631(8) 4_565 ?
Si3 O6 1.648(11) . ?
Si3 O5 1.663(11) . ?
Si4 O14 1.617(8) 1_565 ?
Si4 O14 1.617(8) 4_565 ?
Si4 O15 1.632(15) . ?
Si4 O15 1.632(15) 4_575 ?
Si4 O12 1.674(11) . ?
Si5 O17 1.587(13) . ?
Si5 O16 1.588(12) . ?
Si5 O13 1.642(8) . ?
Si5 O13 1.642(8) 4_565 ?
O10 H1 0.850(10) . ?
O11 H2 0.851(10) . ?
O15 O15 0.76(3) 4_575 ?
 
loop_
 _geom_angle_atom_site_label_1
 _geom_angle_atom_site_label_2
 _geom_angle_atom_site_label_3
 _geom_angle
 _geom_angle_site_symmetry_1
 _geom_angle_site_symmetry_3
 _geom_angle_publ_flag
O3 Ca O3 79.9(4) 1_545 4_575 ?
O3 Ca O7 74.6(3) 1_545 1_655 ?
O3 Ca O7 74.6(3) 4_575 1_655 ?
O3 Ca O1 173.3(3) 1_545 3_666 ?
O3 Ca O1 101.3(3) 4_575 3_666 ?
O7 Ca O1 112.0(3) 1_655 3_666 ?
O3 Ca O1 101.3(3) 1_545 2_646 ?
O3 Ca O1 173.3(3) 4_575 2_646 ?
O7 Ca O1 112.0(3) 1_655 2_646 ?
O1 Ca O1 76.7(4) 3_666 2_646 ?
O3 Ca O5 102.7(3) 1_545 . ?
O3 Ca O5 102.7(3) 4_575 . ?
O7 Ca O5 176.4(4) 1_655 . ?
O1 Ca O5 70.6(3) 3_666 . ?
O1 Ca O5 70.6(3) 2_646 . ?
O3 Ca O6 61.1(2) 1_545 . ?
O3 Ca O6 61.1(2) 4_575 . ?
O7 Ca O6 120.7(3) 1_655 . ?
O1 Ca O6 113.6(2) 3_666 . ?
O1 Ca O6 113.6(2) 2_646 . ?
O5 Ca O6 55.8(3) . . ?
O3 Ca O9 128.9(3) 1_545 . ?
O3 Ca O9 55.8(3) 4_575 . ?
O7 Ca O9 70.3(2) 1_655 . ?
O1 Ca O9 55.6(3) 3_666 . ?
O1 Ca O9 125.7(3) 2_646 . ?
O5 Ca O9 110.3(2) . . ?
O6 Ca O9 108.6(2) . . ?
O3 Ca O9 55.8(3) 1_545 1_545 ?
O3 Ca O9 128.9(3) 4_575 1_545 ?
O7 Ca O9 70.3(2) 1_655 1_545 ?
O1 Ca O9 125.7(3) 3_666 1_545 ?
O1 Ca O9 55.6(3) 2_646 1_545 ?
O5 Ca O9 110.3(2) . 1_545 ?
O6 Ca O9 108.6(2) . 1_545 ?
O9 Ca O9 135.6(4) . 1_545 ?
O3 Ca Si2 102.6(2) 1_545 . ?
O3 Ca Si2 27.06(19) 4_575 . ?
O7 Ca Si2 67.25(12) 1_655 . ?
O1 Ca Si2 80.4(2) 3_666 . ?
O1 Ca Si2 154.8(2) 2_646 . ?
O5 Ca Si2 111.45(12) . . ?
O6 Ca Si2 85.27(13) . . ?
O9 Ca Si2 29.1(2) . . ?
O9 Ca Si2 136.4(2) 1_545 . ?
O3 Ca Si2 27.06(19) 1_545 1_545 ?
O3 Ca Si2 102.6(2) 4_575 1_545 ?
O7 Ca Si2 67.25(12) 1_655 1_545 ?
O1 Ca Si2 154.8(2) 3_666 1_545 ?
O1 Ca Si2 80.4(2) 2_646 1_545 ?
O5 Ca Si2 111.45(12) . 1_545 ?
O6 Ca Si2 85.27(13) . 1_545 ?
O9 Ca Si2 136.4(2) . 1_545 ?
O9 Ca Si2 29.1(2) 1_545 1_545 ?
Si2 Ca Si2 119.30(15) . 1_545 ?
O3 Ca Si1 157.9(2) 1_545 3_666 ?
O3 Ca Si1 80.6(2) 4_575 3_666 ?
O7 Ca Si1 90.28(16) 1_655 3_666 ?
O1 Ca Si1 26.82(19) 3_666 3_666 ?
O1 Ca Si1 99.3(2) 2_646 3_666 ?
O5 Ca Si1 91.62(15) . 3_666 ?
O6 Ca Si1 116.88(10) . 3_666 ?
O9 Ca Si1 29.0(2) . 3_666 ?
O9 Ca Si1 134.2(2) 1_545 3_666 ?
Si2 Ca Si1 56.01(9) . 3_666 ?
Si2 Ca Si1 155.00(14) 1_545 3_666 ?
O7 Ce2 O14 139.43(19) 1_655 . ?
O7 Ce2 O14 139.43(19) 1_655 4_565 ?
O14 Ce2 O14 80.2(4) . 4_565 ?
O7 Ce2 O2 83.2(3) 1_655 1_655 ?
O14 Ce2 O2 118.4(2) . 1_655 ?
O14 Ce2 O2 81.8(2) 4_565 1_655 ?
O7 Ce2 O2 83.2(3) 1_655 4_665 ?
O14 Ce2 O2 81.8(2) . 4_665 ?
O14 Ce2 O2 118.4(2) 4_565 4_665 ?
O2 Ce2 O2 57.4(3) 1_655 4_665 ?
O7 Ce2 O10 113.0(3) 1_655 . ?
O14 Ce2 O10 67.8(2) . . ?
O14 Ce2 O10 67.8(2) 4_565 . ?
O2 Ce2 O10 147.81(19) 1_655 . ?
O2 Ce2 O10 147.81(19) 4_665 . ?
O7 Ce2 O3 67.3(3) 1_655 1_545 ?
O14 Ce2 O3 82.8(2) . 1_545 ?
O14 Ce2 O3 125.4(2) 4_565 1_545 ?
O2 Ce2 O3 149.7(2) 1_655 1_545 ?
O2 Ce2 O3 109.8(2) 4_665 1_545 ?
O10 Ce2 O3 57.7(2) . 1_545 ?
O7 Ce2 O3 67.3(2) 1_655 4_575 ?
O14 Ce2 O3 125.4(2) . 4_575 ?
O14 Ce2 O3 82.8(2) 4_565 4_575 ?
O2 Ce2 O3 109.8(2) 1_655 4_575 ?
O2 Ce2 O3 149.7(2) 4_665 4_575 ?
O10 Ce2 O3 57.7(2) . 4_575 ?
O3 Ce2 O3 66.2(3) 1_545 4_575 ?
O7 Ce2 O8 73.1(2) 1_655 1_545 ?
O14 Ce2 O8 67.2(3) . 1_545 ?
O14 Ce2 O8 147.3(3) 4_565 1_545 ?
O2 Ce2 O8 111.5(3) 1_655 1_545 ?
O2 Ce2 O8 56.7(3) 4_665 1_545 ?
O10 Ce2 O8 100.0(2) . 1_545 ?
O3 Ce2 O8 54.2(3) 1_545 1_545 ?
O3 Ce2 O8 117.2(3) 4_575 1_545 ?
O7 Ce2 O8 73.1(2) 1_655 . ?
O14 Ce2 O8 147.3(3) . . ?
O14 Ce2 O8 67.2(3) 4_565 . ?
O2 Ce2 O8 56.7(3) 1_655 . ?
O2 Ce2 O8 111.5(3) 4_665 . ?
O10 Ce2 O8 100.0(2) . . ?
O3 Ce2 O8 117.2(3) 1_545 . ?
O3 Ce2 O8 54.2(3) 4_575 . ?
O8 Ce2 O8 145.3(4) 1_545 . ?
O7 Ce2 O17 141.5(3) 1_655 1_655 ?
O14 Ce2 O17 57.4(2) . 1_655 ?
O14 Ce2 O17 57.4(2) 4_565 1_655 ?
O2 Ce2 O17 63.3(2) 1_655 1_655 ?
O2 Ce2 O17 63.3(2) 4_665 1_655 ?
O10 Ce2 O17 105.5(3) . 1_655 ?
O3 Ce2 O17 139.9(2) 1_545 1_655 ?
O3 Ce2 O17 139.9(2) 4_575 1_655 ?
O8 Ce2 O17 100.8(2) 1_545 1_655 ?
O8 Ce2 O17 100.8(2) . 1_655 ?
O7 Ce2 Si3 80.9(3) 1_655 1_655 ?
O14 Ce2 Si3 101.97(18) . 1_655 ?
O14 Ce2 Si3 101.97(18) 4_565 1_655 ?
O2 Ce2 Si3 28.71(17) 1_655 1_655 ?
O2 Ce2 Si3 28.71(17) 4_665 1_655 ?
O10 Ce2 Si3 166.1(2) . 1_655 ?
O3 Ce2 Si3 132.31(16) 1_545 1_655 ?
O3 Ce2 Si3 132.31(16) 4_575 1_655 ?
O8 Ce2 Si3 83.7(2) 1_545 1_655 ?
O8 Ce2 Si3 83.7(2) . 1_655 ?
O17 Ce2 Si3 60.6(2) 1_655 1_655 ?
O7 Ce2 Si2 64.08(12) 1_655 1_545 ?
O14 Ce2 Si2 76.74(19) . 1_545 ?
O14 Ce2 Si2 146.0(2) 4_565 1_545 ?
O2 Ce2 Si2 131.43(17) 1_655 1_545 ?
O2 Ce2 Si2 82.74(18) 4_665 1_545 ?
O10 Ce2 Si2 80.38(14) . 1_545 ?
O3 Ce2 Si2 27.12(16) 1_545 1_545 ?
O3 Ce2 Si2 90.38(17) 4_575 1_545 ?
O8 Ce2 Si2 27.5(2) 1_545 1_545 ?
O8 Ce2 Si2 132.9(2) . 1_545 ?
O17 Ce2 Si2 124.80(6) 1_655 1_545 ?
Si3 Ce2 Si2 107.06(7) 1_655 1_545 ?
O7 Ce2 Si2 64.08(12) 1_655 . ?
O14 Ce2 Si2 145.97(19) . . ?
O14 Ce2 Si2 76.74(19) 4_565 . ?
O2 Ce2 Si2 82.74(18) 1_655 . ?
O2 Ce2 Si2 131.43(17) 4_665 . ?
O10 Ce2 Si2 80.38(14) . . ?
O3 Ce2 Si2 90.38(17) 1_545 . ?
O3 Ce2 Si2 27.12(16) 4_575 . ?
O8 Ce2 Si2 132.9(2) 1_545 . ?
O8 Ce2 Si2 27.5(2) . . ?
O17 Ce2 Si2 124.80(6) 1_655 . ?
Si3 Ce2 Si2 107.06(7) 1_655 . ?
Si2 Ce2 Si2 110.37(11) 1_545 . ?
O7 Ce2 Ca 39.1(3) 1_655 . ?
O14 Ce2 Ca 122.28(17) . . ?
O14 Ce2 Ca 122.28(17) 4_565 . ?
O2 Ce2 Ca 117.16(17) 1_655 . ?
O2 Ce2 Ca 117.16(17) 4_665 . ?
O10 Ce2 Ca 73.9(2) . . ?
O3 Ce2 Ca 39.82(16) 1_545 . ?
O3 Ce2 Ca 39.82(16) 4_575 . ?
O8 Ce2 Ca 79.4(2) 1_545 . ?
O8 Ce2 Ca 79.3(2) . . ?
O17 Ce2 Ca 179.4(2) 1_655 . ?
Si3 Ce2 Ca 119.96(9) 1_655 . ?
Si2 Ce2 Ca 55.19(6) 1_545 . ?
Si2 Ce2 Ca 55.19(6) . . ?
O7 Ce2 Si1 17.5(3) 1_655 1_655 ?
O14 Ce2 Si1 138.66(19) . 1_655 ?
O14 Ce2 Si1 138.67(19) 4_565 1_655 ?
O2 Ce2 Si1 68.01(17) 1_655 1_655 ?
O2 Ce2 Si1 68.01(17) 4_665 1_655 ?
O10 Ce2 Si1 130.5(2) . 1_655 ?
O3 Ce2 Si1 81.74(16) 1_545 1_655 ?
O3 Ce2 Si1 81.74(16) 4_575 1_655 ?
O8 Ce2 Si1 72.7(2) 1_545 1_655 ?
O8 Ce2 Si1 72.7(2) . 1_655 ?
O17 Ce2 Si1 124.0(2) 1_655 1_655 ?
Si3 Ce2 Si1 63.35(9) 1_655 1_655 ?
Si2 Ce2 Si1 72.17(7) 1_545 1_655 ?
Si2 Ce2 Si1 72.17(7) . 1_655 ?
Ca Ce2 Si1 56.61(8) . 1_655 ?
O7 Ce2 Fe2 94.1(2) 1_655 . ?
O14 Ce2 Fe2 67.42(17) . . ?
O14 Ce2 Fe2 96.49(18) 4_565 . ?
O2 Ce2 Fe2 173.31(18) 1_655 . ?
O2 Ce2 Fe2 128.54(17) 4_665 . ?
O10 Ce2 Fe2 29.00(15) . . ?
O3 Ce2 Fe2 29.88(16) 1_545 . ?
O3 Ce2 Fe2 63.52(16) 4_575 . ?
O8 Ce2 Fe2 73.3(2) 1_545 . ?
O8 Ce2 Fe2 116.7(2) . . ?
O17 Ce2 Fe2 121.1(2) 1_655 . ?
Si3 Ce2 Fe2 156.87(5) 1_655 . ?
Si2 Ce2 Fe2 51.45(8) 1_545 . ?
Si2 Ce2 Fe2 90.57(8) . . ?
Ca Ce2 Fe2 58.38(7) . . ?
Si1 Ce2 Fe2 110.20(8) 1_655 . ?
O7 Ce2 Fe2 94.1(2) 1_655 4_565 ?
O14 Ce2 Fe2 96.49(18) . 4_565 ?
O14 Ce2 Fe2 67.42(17) 4_565 4_565 ?
O2 Ce2 Fe2 128.54(17) 1_655 4_565 ?
O2 Ce2 Fe2 173.31(18) 4_665 4_565 ?
O10 Ce2 Fe2 29.00(15) . 4_565 ?
O3 Ce2 Fe2 63.52(16) 1_545 4_565 ?
O3 Ce2 Fe2 29.88(16) 4_575 4_565 ?
O8 Ce2 Fe2 116.7(2) 1_545 4_565 ?
O8 Ce2 Fe2 73.3(2) . 4_565 ?
O17 Ce2 Fe2 121.1(2) 1_655 4_565 ?
Si3 Ce2 Fe2 156.87(5) 1_655 4_565 ?
Si2 Ce2 Fe2 90.57(8) 1_545 4_565 ?
Si2 Ce2 Fe2 51.45(8) . 4_565 ?
Ca Ce2 Fe2 58.38(7) . 4_565 ?
Si1 Ce2 Fe2 110.20(8) 1_655 4_565 ?
Fe2 Ce2 Fe2 45.36(10) . 4_565 ?
O17 Ce3 O15 140.2(4) 1_655 2_645 ?
O17 Ce3 O15 140.2(4) 1_655 3_665 ?
O15 Ce3 O15 17.3(7) 2_645 3_665 ?
O17 Ce3 O14 66.2(3) 1_655 4_565 ?
O15 Ce3 O14 89.2(4) 2_645 4_565 ?
O15 Ce3 O14 78.4(4) 3_665 4_565 ?
O17 Ce3 O14 66.2(3) 1_655 . ?
O15 Ce3 O14 78.4(4) 2_645 . ?
O15 Ce3 O14 89.2(4) 3_665 . ?
O14 Ce3 O14 76.8(4) 4_565 . ?
O17 Ce3 O13 105.9(3) 1_655 2_645 ?
O15 Ce3 O13 100.1(4) 2_645 2_645 ?
O15 Ce3 O13 110.6(4) 3_665 2_645 ?
O14 Ce3 O13 170.7(2) 4_565 2_645 ?
O14 Ce3 O13 105.0(3) . 2_645 ?
O17 Ce3 O13 105.9(3) 1_655 3_665 ?
O15 Ce3 O13 110.6(4) 2_645 3_665 ?
O15 Ce3 O13 100.1(4) 3_665 3_665 ?
O14 Ce3 O13 105.0(3) 4_565 3_665 ?
O14 Ce3 O13 170.7(2) . 3_665 ?
O13 Ce3 O13 71.8(3) 2_645 3_665 ?
O17 Ce3 O12 161.2(4) 1_655 3_665 ?
O15 Ce3 O12 58.2(4) 2_645 3_665 ?
O15 Ce3 O12 58.2(4) 3_665 3_665 ?
O14 Ce3 O12 126.8(2) 4_565 3_665 ?
O14 Ce3 O12 126.8(2) . 3_665 ?
O13 Ce3 O12 59.7(2) 2_645 3_665 ?
O13 Ce3 O12 59.7(2) 3_665 3_665 ?
O17 Ce3 O15 114.0(3) 1_655 4_565 ?
O15 Ce3 O15 48.1(6) 2_645 4_565 ?
O15 Ce3 O15 65.3(3) 3_665 4_565 ?
O14 Ce3 O15 115.8(3) 4_565 4_565 ?
O14 Ce3 O15 52.9(3) . 4_565 ?
O13 Ce3 O15 71.4(3) 2_645 4_565 ?
O13 Ce3 O15 131.3(3) 3_665 4_565 ?
O12 Ce3 O15 74.5(3) 3_665 4_565 ?
O17 Ce3 O15 114.0(3) 1_655 . ?
O15 Ce3 O15 65.3(3) 2_645 . ?
O15 Ce3 O15 48.1(6) 3_665 . ?
O14 Ce3 O15 52.9(3) 4_565 . ?
O14 Ce3 O15 115.8(3) . . ?
O13 Ce3 O15 131.3(3) 2_645 . ?
O13 Ce3 O15 71.4(3) 3_665 . ?
O12 Ce3 O15 74.5(3) 3_665 . ?
O15 Ce3 O15 113.2(6) 4_565 . ?
O17 Ce3 O16 53.3(4) 1_655 1_655 ?
O15 Ce3 O16 163.4(4) 2_645 1_655 ?
O15 Ce3 O16 163.4(4) 3_665 1_655 ?
O14 Ce3 O16 107.3(2) 4_565 1_655 ?
O14 Ce3 O16 107.3(2) . 1_655 ?
O13 Ce3 O16 63.4(2) 2_645 1_655 ?
O13 Ce3 O16 63.4(2) 3_665 1_655 ?
O12 Ce3 O16 107.9(3) 3_665 1_655 ?
O15 Ce3 O16 122.7(3) 4_565 1_655 ?
O15 Ce3 O16 122.7(3) . 1_655 ?
O17 Ce3 Si4 168.4(3) 1_655 3_665 ?
O15 Ce3 Si4 28.7(3) 2_645 3_665 ?
O15 Ce3 Si4 28.7(3) 3_665 3_665 ?
O14 Ce3 Si4 105.14(18) 4_565 3_665 ?
O14 Ce3 Si4 105.14(18) . 3_665 ?
O13 Ce3 Si4 83.37(17) 2_645 3_665 ?
O13 Ce3 Si4 83.37(17) 3_665 3_665 ?
O12 Ce3 Si4 30.3(2) 3_665 3_665 ?
O15 Ce3 Si4 61.8(3) 4_565 3_665 ?
O15 Ce3 Si4 61.8(3) . 3_665 ?
O16 Ce3 Si4 138.3(2) 1_655 3_665 ?
O17 Ce3 O16 66.2(2) 1_655 3_665 ?
O15 Ce3 O16 129.3(4) 2_645 3_665 ?
O15 Ce3 O16 112.0(4) 3_665 3_665 ?
O14 Ce3 O16 60.8(3) 4_565 3_665 ?
O14 Ce3 O16 125.5(3) . 3_665 ?
O13 Ce3 O16 112.2(3) 2_645 3_665 ?
O13 Ce3 O16 50.8(3) 3_665 3_665 ?
O12 Ce3 O16 106.4(2) 3_665 3_665 ?
O15 Ce3 O16 176.3(4) 4_565 3_665 ?
O15 Ce3 O16 64.0(4) . 3_665 ?
O16 Ce3 O16 60.6(2) 1_655 3_665 ?
Si4 Ce3 O16 117.2(2) 3_665 3_665 ?
O17 Ce3 O16 66.2(2) 1_655 3_655 ?
O15 Ce3 O16 112.0(4) 2_645 3_655 ?
O15 Ce3 O16 129.3(4) 3_665 3_655 ?
O14 Ce3 O16 125.5(3) 4_565 3_655 ?
O14 Ce3 O16 60.8(3) . 3_655 ?
O13 Ce3 O16 50.8(3) 2_645 3_655 ?
O13 Ce3 O16 112.2(3) 3_665 3_655 ?
O12 Ce3 O16 106.4(2) 3_665 3_655 ?
O15 Ce3 O16 64.0(4) 4_565 3_655 ?
O15 Ce3 O16 176.3(4) . 3_655 ?
O16 Ce3 O16 60.6(2) 1_655 3_655 ?
Si4 Ce3 O16 117.2(2) 3_665 3_655 ?
O16 Ce3 O16 118.7(4) 3_665 3_655 ?
O17 Ce3 Si5 25.5(3) 1_655 1_655 ?
O15 Ce3 Si5 164.0(3) 2_645 1_655 ?
O15 Ce3 Si5 164.0(3) 3_665 1_655 ?
O14 Ce3 Si5 85.69(18) 4_565 1_655 ?
O14 Ce3 Si5 85.69(18) . 1_655 ?
O13 Ce3 Si5 85.33(17) 2_645 1_655 ?
O13 Ce3 Si5 85.33(17) 3_665 1_655 ?
O12 Ce3 Si5 135.7(2) 3_665 1_655 ?
O15 Ce3 Si5 121.8(3) 4_565 1_655 ?
O15 Ce3 Si5 121.8(3) . 1_655 ?
O16 Ce3 Si5 27.8(2) 1_655 1_655 ?
Si4 Ce3 Si5 166.03(11) 3_665 1_655 ?
O16 Ce3 Si5 60.1(2) 3_665 1_655 ?
O16 Ce3 Si5 60.1(2) 3_655 1_655 ?
O17 Ce3 Si4 88.57(19) 1_655 1_545 ?
O15 Ce3 Si4 62.5(3) 2_645 1_545 ?
O15 Ce3 Si4 77.5(3) 3_665 1_545 ?
O14 Ce3 Si4 96.44(19) 4_565 1_545 ?
O14 Ce3 Si4 25.3(2) . 1_545 ?
O13 Ce3 Si4 88.00(18) 2_645 1_545 ?
O13 Ce3 Si4 157.62(18) 3_665 1_545 ?
O12 Ce3 Si4 102.04(14) 3_665 1_545 ?
O15 Ce3 Si4 27.7(3) 4_565 1_545 ?
O15 Ce3 Si4 118.7(3) . 1_545 ?
O16 Ce3 Si4 116.49(11) 1_655 1_545 ?
Si4 Ce3 Si4 84.79(9) 3_665 1_545 ?
O16 Ce3 Si4 150.8(2) 3_665 1_545 ?
O16 Ce3 Si4 57.7(2) 3_655 1_545 ?
Si5 Ce3 Si4 103.02(8) 1_655 1_545 ?
O17 Ce3 Si4 88.57(19) 1_655 . ?
O15 Ce3 Si4 77.5(3) 2_645 . ?
O15 Ce3 Si4 62.5(3) 3_665 . ?
O14 Ce3 Si4 25.3(2) 4_565 . ?
O14 Ce3 Si4 96.44(19) . . ?
O13 Ce3 Si4 157.62(18) 2_645 . ?
O13 Ce3 Si4 88.00(18) 3_665 . ?
O12 Ce3 Si4 102.04(14) 3_665 . ?
O15 Ce3 Si4 118.7(3) 4_565 . ?
O15 Ce3 Si4 27.7(3) . . ?
O16 Ce3 Si4 116.49(11) 1_655 . ?
Si4 Ce3 Si4 84.79(8) 3_665 . ?
O16 Ce3 Si4 57.7(2) 3_665 . ?
O16 Ce3 Si4 150.8(2) 3_655 . ?
Si5 Ce3 Si4 103.02(8) 1_655 . ?
Si4 Ce3 Si4 109.75(12) 1_545 . ?
O17 Ce3 Si5 86.86(19) 1_655 3_655 ?
O15 Ce3 Si5 107.1(3) 2_645 3_655 ?
O15 Ce3 Si5 122.3(3) 3_665 3_655 ?
O14 Ce3 Si5 151.1(2) 4_565 3_655 ?
O14 Ce3 Si5 83.18(19) . 3_655 ?
O13 Ce3 Si5 24.58(17) 2_645 3_655 ?
O13 Ce3 Si5 91.70(18) 3_665 3_655 ?
O12 Ce3 Si5 81.94(14) 3_665 3_655 ?
O15 Ce3 Si5 64.8(3) 4_565 3_655 ?
O15 Ce3 Si5 155.7(3) . 3_655 ?
O16 Ce3 Si5 59.25(10) 1_655 3_655 ?
Si4 Ce3 Si5 99.98(8) 3_665 3_655 ?
O16 Ce3 Si5 118.7(2) 3_665 3_655 ?
O16 Ce3 Si5 26.3(2) 3_655 3_655 ?
Si5 Ce3 Si5 72.14(8) 1_655 3_655 ?
Si4 Ce3 Si5 71.76(8) 1_545 3_655 ?
Si4 Ce3 Si5 175.16(9) . 3_655 ?
O17 Ce3 Si5 86.86(19) 1_655 3_665 ?
O15 Ce3 Si5 122.3(3) 2_645 3_665 ?
O15 Ce3 Si5 107.1(3) 3_665 3_665 ?
O14 Ce3 Si5 83.18(19) 4_565 3_665 ?
O14 Ce3 Si5 151.1(2) . 3_665 ?
O13 Ce3 Si5 91.70(18) 2_645 3_665 ?
O13 Ce3 Si5 24.58(17) 3_665 3_665 ?
O12 Ce3 Si5 81.94(14) 3_665 3_665 ?
O15 Ce3 Si5 155.7(3) 4_565 3_665 ?
O15 Ce3 Si5 64.8(3) . 3_665 ?
O16 Ce3 Si5 59.25(10) 1_655 3_665 ?
Si4 Ce3 Si5 99.98(8) 3_665 3_665 ?
O16 Ce3 Si5 26.3(2) 3_665 3_665 ?
O16 Ce3 Si5 118.7(2) 3_655 3_665 ?
Si5 Ce3 Si5 72.14(8) 1_655 3_665 ?
Si4 Ce3 Si5 175.16(9) 1_545 3_665 ?
Si4 Ce3 Si5 71.76(8) . 3_665 ?
Si5 Ce3 Si5 106.36(11) 3_655 3_665 ?
O17 Ce3 O15 109.5(3) 1_655 1_545 ?
O15 Ce3 O15 54.6(3) 2_645 1_545 ?
O15 Ce3 O15 71.9(5) 3_665 1_545 ?
O14 Ce3 O15 119.1(3) 4_565 1_545 ?
O14 Ce3 O15 51.4(3) . 1_545 ?
O13 Ce3 O15 67.4(3) 2_645 1_545 ?
O13 Ce3 O15 131.5(3) 3_665 1_545 ?
O12 Ce3 O15 77.4(2) 3_665 1_545 ?
O15 Ce3 O15 6.6(3) 4_565 1_545 ?
O15 Ce3 O15 119.8(5) . 1_545 ?
O16 Ce3 O15 116.2(3) 1_655 1_545 ?
Si4 Ce3 O15 67.2(2) 3_665 1_545 ?
O16 Ce3 O15 175.6(3) 3_665 1_545 ?
O16 Ce3 O15 57.4(3) 3_655 1_545 ?
Si5 Ce3 O15 115.6(2) 1_655 1_545 ?
Si4 Ce3 O15 26.4(2) 1_545 1_545 ?
Si4 Ce3 O15 124.4(3) . 1_545 ?
Si5 Ce3 O15 59.0(3) 3_655 1_545 ?
Si5 Ce3 O15 156.0(2) 3_665 1_545 ?
O16 Ce4 O2 141.00(19) 3_565 . ?
O16 Ce4 O2 141.00(19) 3_565 4_575 ?
O2 Ce4 O2 77.4(4) . 4_575 ?
O16 Ce4 O11 123.2(4) 3_565 . ?
O2 Ce4 O11 68.6(2) . . ?
O2 Ce4 O11 68.6(2) 4_575 . ?
O16 Ce4 O14 75.3(4) 3_565 4_465 ?
O2 Ce4 O14 80.6(3) . 4_465 ?
O2 Ce4 O14 115.7(2) 4_575 4_465 ?
O11 Ce4 O14 147.4(2) . 4_465 ?
O16 Ce4 O14 75.3(4) 3_565 1_465 ?
O2 Ce4 O14 115.7(2) . 1_465 ?
O2 Ce4 O14 80.6(3) 4_575 1_465 ?
O11 Ce4 O14 147.4(2) . 1_465 ?
O14 Ce4 O14 57.0(3) 4_465 1_465 ?
O16 Ce4 O13 74.0(3) 3_565 . ?
O2 Ce4 O13 86.1(2) . . ?
O2 Ce4 O13 127.7(2) 4_575 . ?
O11 Ce4 O13 59.1(2) . . ?
O14 Ce4 O13 109.8(2) 4_465 . ?
O14 Ce4 O13 149.0(2) 1_465 . ?
O16 Ce4 O13 74.0(3) 3_565 4_575 ?
O2 Ce4 O13 127.7(2) . 4_575 ?
O2 Ce4 O13 86.1(2) 4_575 4_575 ?
O11 Ce4 O13 59.1(2) . 4_575 ?
O14 Ce4 O13 149.0(2) 4_465 4_575 ?
O14 Ce4 O13 109.8(2) 1_465 4_575 ?
O13 Ce4 O13 65.8(3) . 4_575 ?
O16 Ce4 O17 74.5(2) 3_565 1_565 ?
O2 Ce4 O17 144.0(3) . 1_565 ?
O2 Ce4 O17 66.7(3) 4_575 1_565 ?
O11 Ce4 O17 99.2(2) . 1_565 ?
O14 Ce4 O17 112.3(3) 4_465 1_565 ?
O14 Ce4 O17 57.3(3) 1_465 1_565 ?
O13 Ce4 O17 117.5(3) . 1_565 ?
O13 Ce4 O17 54.2(3) 4_575 1_565 ?
O16 Ce4 O17 74.5(2) 3_565 . ?
O2 Ce4 O17 66.7(3) . . ?
O2 Ce4 O17 144.0(3) 4_575 . ?
O11 Ce4 O17 99.2(2) . . ?
O14 Ce4 O17 57.3(3) 4_465 . ?
O14 Ce4 O17 112.3(3) 1_465 . ?
O13 Ce4 O17 54.2(3) . . ?
O13 Ce4 O17 117.5(3) 4_575 . ?
O17 Ce4 O17 148.9(5) 1_565 . ?
O16 Ce4 O8 131.3(4) 3_565 1_455 ?
O2 Ce4 O8 55.4(2) . 1_455 ?
O2 Ce4 O8 55.4(2) 4_575 1_455 ?
O11 Ce4 O8 105.5(3) . 1_455 ?
O14 Ce4 O8 62.3(2) 4_465 1_455 ?
O14 Ce4 O8 62.3(2) 1_465 1_455 ?
O13 Ce4 O8 141.01(19) . 1_455 ?
O13 Ce4 O8 141.01(19) 4_575 1_455 ?
O17 Ce4 O8 99.5(2) 1_565 1_455 ?
O17 Ce4 O8 99.5(2) . 1_455 ?
O16 Ce4 Si4 69.2(4) 3_565 1_455 ?
O2 Ce4 Si4 102.01(17) . 1_455 ?
O2 Ce4 Si4 102.01(17) 4_575 1_455 ?
O11 Ce4 Si4 167.6(2) . 1_455 ?
O14 Ce4 Si4 28.75(17) 4_465 1_455 ?
O14 Ce4 Si4 28.75(18) 1_465 1_455 ?
O13 Ce4 Si4 130.06(16) . 1_455 ?
O13 Ce4 Si4 130.06(16) 4_575 1_455 ?
O17 Ce4 Si4 83.7(2) 1_565 1_455 ?
O17 Ce4 Si4 83.7(2) . 1_455 ?
O8 Ce4 Si4 62.1(2) 1_455 1_455 ?
O16 Ce4 Fe3 165.6(4) 3_565 . ?
O2 Ce4 Fe3 39.57(18) . . ?
O2 Ce4 Fe3 39.57(18) 4_575 . ?
O11 Ce4 Fe3 71.2(2) . . ?
O14 Ce4 Fe3 92.07(18) 4_465 . ?
O14 Ce4 Fe3 92.07(18) 1_465 . ?
O13 Ce4 Fe3 117.62(16) . . ?
O13 Ce4 Fe3 117.62(16) 4_575 . ?
O17 Ce4 Fe3 104.8(2) 1_565 . ?
O17 Ce4 Fe3 104.8(2) . . ?
O8 Ce4 Fe3 34.3(2) 1_455 . ?
Si4 Ce4 Fe3 96.42(9) 1_455 . ?
O16 Ce4 Si5 67.89(19) 3_565 . ?
O2 Ce4 Si5 78.86(19) . . ?
O2 Ce4 Si5 147.07(19) 4_575 . ?
O11 Ce4 Si5 81.65(14) . . ?
O14 Ce4 Si5 82.19(18) 4_465 . ?
O14 Ce4 Si5 130.7(2) 1_465 . ?
O13 Ce4 Si5 27.70(16) . . ?
O13 Ce4 Si5 90.70(17) 4_575 . ?
O17 Ce4 Si5 134.6(3) 1_565 . ?
O17 Ce4 Si5 27.2(2) . . ?
O8 Ce4 Si5 124.32(6) 1_455 . ?
Si4 Ce4 Si5 105.00(8) 1_455 . ?
Fe3 Ce4 Si5 117.96(6) . . ?
O16 Ce4 Si5 67.89(19) 3_565 1_565 ?
O2 Ce4 Si5 147.07(19) . 1_565 ?
O2 Ce4 Si5 78.86(19) 4_575 1_565 ?
O11 Ce4 Si5 81.65(14) . 1_565 ?
O14 Ce4 Si5 130.7(2) 4_465 1_565 ?
O14 Ce4 Si5 82.19(18) 1_465 1_565 ?
O13 Ce4 Si5 90.70(17) . 1_565 ?
O13 Ce4 Si5 27.70(16) 4_575 1_565 ?
O17 Ce4 Si5 27.2(2) 1_565 1_565 ?
O17 Ce4 Si5 134.6(3) . 1_565 ?
O8 Ce4 Si5 124.32(6) 1_455 1_565 ?
Si4 Ce4 Si5 105.00(8) 1_455 1_565 ?
Fe3 Ce4 Si5 117.96(6) . 1_565 ?
Si5 Ce4 Si5 111.35(12) . 1_565 ?
O16 Ce4 Fe2 103.1(4) 3_565 1_565 ?
O2 Ce4 Fe2 97.72(18) . 1_565 ?
O2 Ce4 Fe2 69.05(17) 4_575 1_565 ?
O11 Ce4 Fe2 29.58(14) . 1_565 ?
O14 Ce4 Fe2 174.25(18) 4_465 1_565 ?
O14 Ce4 Fe2 128.28(18) 1_465 1_565 ?
O13 Ce4 Fe2 64.53(16) . 1_565 ?
O13 Ce4 Fe2 30.92(16) 4_575 1_565 ?
O17 Ce4 Fe2 72.3(2) 1_565 1_565 ?
O17 Ce4 Fe2 117.0(2) . 1_565 ?
O8 Ce4 Fe2 121.3(2) 1_455 1_565 ?
Si4 Ce4 Fe2 155.98(5) 1_455 1_565 ?
Fe3 Ce4 Fe2 90.08(7) . 1_565 ?
Si5 Ce4 Fe2 92.09(8) . 1_565 ?
Si5 Ce4 Fe2 52.15(8) 1_565 1_565 ?
O16 Ce4 Fe2 103.1(4) 3_565 4_565 ?
O2 Ce4 Fe2 69.04(17) . 4_565 ?
O2 Ce4 Fe2 97.72(18) 4_575 4_565 ?
O11 Ce4 Fe2 29.58(14) . 4_565 ?
O14 Ce4 Fe2 128.28(18) 4_465 4_565 ?
O14 Ce4 Fe2 174.25(18) 1_465 4_565 ?
O13 Ce4 Fe2 30.92(16) . 4_565 ?
O13 Ce4 Fe2 64.53(16) 4_575 4_565 ?
O17 Ce4 Fe2 117.0(2) 1_565 4_565 ?
O17 Ce4 Fe2 72.3(2) . 4_565 ?
O8 Ce4 Fe2 121.3(2) 1_455 4_565 ?
Si4 Ce4 Fe2 155.98(5) 1_455 4_565 ?
Fe3 Ce4 Fe2 90.08(7) . 4_565 ?
Si5 Ce4 Fe2 52.15(8) . 4_565 ?
Si5 Ce4 Fe2 92.09(8) 1_565 4_565 ?
Fe2 Ce4 Fe2 46.35(10) 1_565 4_565 ?
O16 Ce4 Si3 128.67(11) 3_565 1_565 ?
O2 Ce4 Si3 90.07(19) . 1_565 ?
O2 Ce4 Si3 19.25(18) 4_575 1_565 ?
O11 Ce4 Si3 59.67(12) . 1_565 ?
O14 Ce4 Si3 133.04(18) 4_465 1_565 ?
O14 Ce4 Si3 87.77(19) 1_465 1_565 ?
O13 Ce4 Si3 115.38(16) . 1_565 ?
O13 Ce4 Si3 66.85(17) 4_575 1_565 ?
O17 Ce4 Si3 56.0(2) 1_565 1_565 ?
O17 Ce4 Si3 154.0(2) . 1_565 ?
O8 Ce4 Si3 74.54(14) 1_455 1_565 ?
Si4 Ce4 Si3 113.81(7) 1_455 1_565 ?
Fe3 Ce4 Si3 56.16(6) . 1_565 ?
Si5 Ce4 Si3 141.08(9) . 1_565 ?
Si5 Ce4 Si3 61.90(8) 1_565 1_565 ?
Fe2 Ce4 Si3 52.22(8) 1_565 1_565 ?
Fe2 Ce4 Si3 89.00(8) 4_565 1_565 ?
O4 Fe1 O4 180.0 . 3_666 ?
O4 Fe1 O1 92.6(4) . 3_666 ?
O4 Fe1 O1 87.4(4) 3_666 3_666 ?
O4 Fe1 O1 87.4(4) . . ?
O4 Fe1 O1 92.6(4) 3_666 . ?
O1 Fe1 O1 180.0(4) 3_666 . ?
O4 Fe1 O5 85.0(3) . 3_666 ?
O4 Fe1 O5 95.0(3) 3_666 3_666 ?
O1 Fe1 O5 90.2(4) 3_666 3_666 ?
O1 Fe1 O5 89.8(4) . 3_666 ?
O4 Fe1 O5 95.0(3) . . ?
O4 Fe1 O5 85.0(3) 3_666 . ?
O1 Fe1 O5 89.8(4) 3_666 . ?
O1 Fe1 O5 90.2(4) . . ?
O5 Fe1 O5 180.0 3_666 . ?
O4 Fe1 Fe1 40.2(3) . 2_656 ?
O4 Fe1 Fe1 139.8(3) 3_666 2_656 ?
O1 Fe1 Fe1 88.5(2) 3_666 2_656 ?
O1 Fe1 Fe1 91.5(2) . 2_656 ?
O5 Fe1 Fe1 45.0(2) 3_666 2_656 ?
O5 Fe1 Fe1 135.0(2) . 2_656 ?
O4 Fe1 Fe1 139.8(3) . 2_646 ?
O4 Fe1 Fe1 40.2(3) 3_666 2_646 ?
O1 Fe1 Fe1 91.5(2) 3_666 2_646 ?
O1 Fe1 Fe1 88.5(2) . 2_646 ?
O5 Fe1 Fe1 135.0(2) 3_666 2_646 ?
O5 Fe1 Fe1 45.0(2) . 2_646 ?
Fe1 Fe1 Fe1 180.0 2_656 2_646 ?
O4 Fe1 Ca 91.8(3) . . ?
O4 Fe1 Ca 88.2(3) 3_666 . ?
O1 Fe1 Ca 42.8(2) 3_666 . ?
O1 Fe1 Ca 137.2(2) . . ?
O5 Fe1 Ca 132.8(3) 3_666 . ?
O5 Fe1 Ca 47.2(3) . . ?
Fe1 Fe1 Ca 114.61(2) 2_656 . ?
Fe1 Fe1 Ca 65.39(2) 2_646 . ?
O10 Fe2 O11 179.9(4) . 1_545 ?
O10 Fe2 O3 88.5(4) . 1_545 ?
O11 Fe2 O3 91.5(4) 1_545 1_545 ?
O10 Fe2 O13 91.3(4) . 4_565 ?
O11 Fe2 O13 88.7(4) 1_545 4_565 ?
O3 Fe2 O13 179.2(4) 1_545 4_565 ?
O10 Fe2 O6 82.7(4) . . ?
O11 Fe2 O6 97.3(3) 1_545 . ?
O3 Fe2 O6 90.1(4) 1_545 . ?
O13 Fe2 O6 90.6(4) 4_565 . ?
O10 Fe2 O12 97.1(4) . 1_545 ?
O11 Fe2 O12 83.0(3) 1_545 1_545 ?
O3 Fe2 O12 91.7(4) 1_545 1_545 ?
O13 Fe2 O12 87.5(4) 4_565 1_545 ?
O6 Fe2 O12 178.1(4) . 1_545 ?
O10 Fe2 Fe2 40.4(3) . 4_565 ?
O11 Fe2 Fe2 139.5(2) 1_545 4_565 ?
O3 Fe2 Fe2 92.4(3) 1_545 4_565 ?
O13 Fe2 Fe2 88.0(3) 4_565 4_565 ?
O6 Fe2 Fe2 42.5(2) . 4_565 ?
O12 Fe2 Fe2 137.1(2) 1_545 4_565 ?
O10 Fe2 Fe2 139.6(3) . 4 ?
O11 Fe2 Fe2 40.5(2) 1_545 4 ?
O3 Fe2 Fe2 87.6(3) 1_545 4 ?
O13 Fe2 Fe2 92.0(3) 4_565 4 ?
O6 Fe2 Fe2 137.5(2) . 4 ?
O12 Fe2 Fe2 42.9(2) 1_545 4 ?
Fe2 Fe2 Fe2 180.0 4_565 4 ?
O10 Fe2 Ca 84.9(3) . . ?
O11 Fe2 Ca 95.0(3) 1_545 . ?
O3 Fe2 Ca 36.2(2) 1_545 . ?
O13 Fe2 Ca 144.5(3) 4_565 . ?
O6 Fe2 Ca 53.9(3) . . ?
O12 Fe2 Ca 128.0(3) 1_545 . ?
Fe2 Fe2 Ca 66.58(6) 4_565 . ?
Fe2 Fe2 Ca 113.41(6) 4 . ?
O10 Fe2 Ce4 137.0(3) . 1_545 ?
O11 Fe2 Ce4 42.9(3) 1_545 1_545 ?
O3 Fe2 Ce4 132.3(3) 1_545 1_545 ?
O13 Fe2 Ce4 48.1(2) 4_565 1_545 ?
O6 Fe2 Ce4 84.3(3) . 1_545 ?
O12 Fe2 Ce4 94.7(3) 1_545 1_545 ?
Fe2 Fe2 Ce4 113.17(5) 4_565 1_545 ?
Fe2 Fe2 Ce4 66.83(5) 4 1_545 ?
Ca Fe2 Ce4 118.60(10) . 1_545 ?
O10 Fe2 Ce2 44.2(3) . . ?
O11 Fe2 Ce2 135.8(3) 1_545 . ?
O3 Fe2 Ce2 46.4(2) 1_545 . ?
O13 Fe2 Ce2 133.2(3) 4_565 . ?
O6 Fe2 Ce2 95.5(3) . . ?
O12 Fe2 Ce2 85.6(3) 1_545 . ?
Fe2 Fe2 Ce2 67.32(5) 4_565 . ?
Fe2 Fe2 Ce2 112.68(5) 4 . ?
Ca Fe2 Ce2 60.28(7) . . ?
Ce4 Fe2 Ce2 178.62(10) 1_545 . ?
O8 Fe3 O4 167.2(5) 1_455 . ?
O8 Fe3 O2 81.9(3) 1_455 4_575 ?
O4 Fe3 O2 89.3(3) . 4_575 ?
O8 Fe3 O2 82.0(3) 1_455 . ?
O4 Fe3 O2 89.3(3) . . ?
O2 Fe3 O2 93.3(4) 4_575 . ?
O8 Fe3 O1 111.4(3) 1_455 4_575 ?
O4 Fe3 O1 77.9(3) . 4_575 ?
O2 Fe3 O1 90.9(3) 4_575 4_575 ?
O2 Fe3 O1 166.5(3) . 4_575 ?
O8 Fe3 O1 111.4(3) 1_455 . ?
O4 Fe3 O1 77.9(3) . . ?
O2 Fe3 O1 166.5(3) 4_575 . ?
O2 Fe3 O1 90.9(3) . . ?
O1 Fe3 O1 82.2(4) 4_575 . ?
O8 Fe3 Ce4 66.2(3) 1_455 . ?
O4 Fe3 Ce4 101.0(3) . . ?
O2 Fe3 Ce4 47.8(2) 4_575 . ?
O2 Fe3 Ce4 47.8(2) . . ?
O1 Fe3 Ce4 138.6(2) 4_575 . ?
O1 Fe3 Ce4 138.6(2) . . ?
O8 Fe3 Ce 109.2(4) 1_455 3_666 ?
O4 Fe3 Ce 83.6(3) . 3_666 ?
O2 Fe3 Ce 132.9(2) 4_575 3_666 ?
O2 Fe3 Ce 132.9(2) . 3_666 ?
O1 Fe3 Ce 42.0(2) 4_575 3_666 ?
O1 Fe3 Ce 42.0(2) . 3_666 ?
Ce4 Fe3 Ce 175.40(10) . 3_666 ?
O8 Fe3 Ce2 49.43(9) 1_455 1_455 ?
O4 Fe3 Ce2 126.50(14) . 1_455 ?
O2 Fe3 Ce2 109.0(2) 4_575 1_455 ?
O2 Fe3 Ce2 41.6(2) . 1_455 ?
O1 Fe3 Ce2 147.1(2) 4_575 1_455 ?
O1 Fe3 Ce2 82.5(2) . 1_455 ?
Ce4 Fe3 Ce2 64.86(4) . 1_455 ?
Ce Fe3 Ce2 112.43(6) 3_666 1_455 ?
O8 Fe3 Ce2 49.43(9) 1_455 1_465 ?
O4 Fe3 Ce2 126.50(14) . 1_465 ?
O2 Fe3 Ce2 41.6(2) 4_575 1_465 ?
O2 Fe3 Ce2 109.0(2) . 1_465 ?
O1 Fe3 Ce2 82.47(19) 4_575 1_465 ?
O1 Fe3 Ce2 147.1(2) . 1_465 ?
Ce4 Fe3 Ce2 64.86(4) . 1_465 ?
Ce Fe3 Ce2 112.43(6) 3_666 1_465 ?
Ce2 Fe3 Ce2 95.21(6) 1_455 1_465 ?
O8 Fe3 Ce 51.0(2) 1_455 1_455 ?
O4 Fe3 Ce 137.4(2) . 1_455 ?
O2 Fe3 Ce 132.9(2) 4_575 1_455 ?
O2 Fe3 Ce 83.5(2) . 1_455 ?
O1 Fe3 Ce 103.0(2) 4_575 1_455 ?
O1 Fe3 Ce 60.4(2) . 1_455 ?
Ce4 Fe3 Ce 104.61(6) . 1_455 ?
Ce Fe3 Ce 71.61(7) 3_666 1_455 ?
Ce2 Fe3 Ce 44.40(4) 1_455 1_455 ?
Ce2 Fe3 Ce 95.33(6) 1_465 1_455 ?
O7 Si1 O1 110.7(4) . . ?
O7 Si1 O1 110.7(4) . 4_565 ?
O1 Si1 O1 114.3(6) . 4_565 ?
O7 Si1 O9 107.9(6) . 3_666 ?
O1 Si1 O9 106.5(4) . 3_666 ?
O1 Si1 O9 106.5(4) 4_565 3_666 ?
O7 Si1 Ce 116.49(15) . 3_666 ?
O1 Si1 Ce 41.1(3) . 3_666 ?
O1 Si1 Ce 132.2(3) 4_565 3_666 ?
O9 Si1 Ce 66.01(18) 3_666 3_666 ?
O7 Si1 Ce 116.49(15) . 3_656 ?
O1 Si1 Ce 132.2(3) . 3_656 ?
O1 Si1 Ce 41.1(3) 4_565 3_656 ?
O9 Si1 Ce 66.01(17) 3_666 3_656 ?
Ce Si1 Ce 116.21(14) 3_666 3_656 ?
O7 Si1 Ce 35.2(4) . 1_455 ?
O1 Si1 Ce 121.7(3) . 1_455 ?
O1 Si1 Ce 121.7(3) 4_565 1_455 ?
O9 Si1 Ce 72.7(4) 3_666 1_455 ?
Ce Si1 Ce 101.61(10) 3_666 1_455 ?
Ce Si1 Ce 101.61(10) 3_656 1_455 ?
O7 Si1 Ce2 26.4(4) . 1_455 ?
O1 Si1 Ce2 97.7(3) . 1_455 ?
O1 Si1 Ce2 97.7(3) 4_565 1_455 ?
O9 Si1 Ce2 134.3(4) 3_666 1_455 ?
Ce Si1 Ce2 121.70(7) 3_666 1_455 ?
Ce Si1 Ce2 121.70(7) 3_656 1_455 ?
Ce Si1 Ce2 61.55(8) 1_455 1_455 ?
O8 Si2 O9 110.3(7) . . ?
O8 Si2 O3 108.7(4) . . ?
O9 Si2 O3 108.2(4) . . ?
O8 Si2 O3 108.7(4) . 4_575 ?
O9 Si2 O3 108.2(4) . 4_575 ?
O3 Si2 O3 112.9(6) . 4_575 ?
O8 Si2 Ce 116.43(15) . 1_565 ?
O9 Si2 Ce 67.76(18) . 1_565 ?
O3 Si2 Ce 41.1(3) . 1_565 ?
O3 Si2 Ce 133.2(3) 4_575 1_565 ?
O8 Si2 Ca 116.43(15) . . ?
O9 Si2 Ca 67.76(18) . . ?
O3 Si2 Ca 133.2(3) . . ?
O3 Si2 Ca 41.1(3) 4_575 . ?
Ce Si2 Ca 119.30(15) 1_565 . ?
O8 Si2 Ce2 59.17(14) . . ?
O9 Si2 Ce2 114.4(2) . . ?
O3 Si2 Ce2 137.3(3) . . ?
O3 Si2 Ce2 50.7(3) 4_575 . ?
Ce Si2 Ce2 175.39(12) 1_565 . ?
Ca Si2 Ce2 65.15(4) . . ?
O8 Si2 Ce2 59.17(14) . 1_565 ?
O9 Si2 Ce2 114.4(2) . 1_565 ?
O3 Si2 Ce2 50.7(3) . 1_565 ?
O3 Si2 Ce2 137.3(3) 4_575 1_565 ?
Ce Si2 Ce2 65.15(4) 1_565 1_565 ?
Ca Si2 Ce2 175.39(12) . 1_565 ?
Ce2 Si2 Ce2 110.36(11) . 1_565 ?
O8 Si2 Ce 77.5(5) . 3_766 ?
O9 Si2 Ce 32.8(4) . 3_766 ?
O3 Si2 Ce 120.6(3) . 3_766 ?
O3 Si2 Ce 120.6(3) 4_575 3_766 ?
Ce Si2 Ce 82.14(9) 1_565 3_766 ?
Ca Si2 Ce 82.14(9) . 3_766 ?
Ce2 Si2 Ce 97.73(7) . 3_766 ?
Ce2 Si2 Ce 97.73(7) 1_565 3_766 ?
O8 Si2 Ce4 19.2(4) . 1_655 ?
O9 Si2 Ce4 129.4(5) . 1_655 ?
O3 Si2 Ce4 98.9(3) . 1_655 ?
O3 Si2 Ce4 98.9(3) 4_575 1_655 ?
Ce Si2 Ce4 119.93(7) 1_565 1_655 ?
Ca Si2 Ce4 119.93(7) . 1_655 ?
Ce2 Si2 Ce4 55.48(6) . 1_655 ?
Ce2 Si2 Ce4 55.48(6) 1_565 1_655 ?
Ce Si2 Ce4 96.62(8) 3_766 1_655 ?
O2 Si3 O2 103.9(6) . 4_565 ?
O2 Si3 O6 112.8(4) . . ?
O2 Si3 O6 112.8(4) 4_565 . ?
O2 Si3 O5 112.8(4) . . ?
O2 Si3 O5 112.8(4) 4_565 . ?
O6 Si3 O5 102.0(6) . . ?
O2 Si3 Ce2 52.0(3) . 1_455 ?
O2 Si3 Ce2 52.0(3) 4_565 1_455 ?
O6 Si3 Ce2 132.3(4) . 1_455 ?
O5 Si3 Ce2 125.8(4) . 1_455 ?
O2 Si3 Ca 127.7(3) . . ?
O2 Si3 Ca 127.7(3) 4_565 . ?
O6 Si3 Ca 57.5(4) . . ?
O5 Si3 Ca 44.5(4) . . ?
Ce2 Si3 Ca 170.26(14) 1_455 . ?
O2 Si3 Ce4 109.4(3) . 1_545 ?
O2 Si3 Ce4 30.7(3) 4_565 1_545 ?
O6 Si3 Ce4 83.4(2) . 1_545 ?
O5 Si3 Ce4 130.85(5) . 1_545 ?
Ce2 Si3 Ce4 66.43(6) 1_455 1_545 ?
Ca Si3 Ce4 118.80(8) . 1_545 ?
O2 Si3 Ce4 30.7(3) . . ?
O2 Si3 Ce4 109.4(3) 4_565 . ?
O6 Si3 Ce4 83.4(2) . . ?
O5 Si3 Ce4 130.85(5) . . ?
Ce2 Si3 Ce4 66.43(6) 1_455 . ?
Ca Si3 Ce4 118.80(8) . . ?
Ce4 Si3 Ce4 98.25(9) 1_545 . ?
O2 Si3 Ce3 62.1(3) . 1_455 ?
O2 Si3 Ce3 62.1(3) 4_565 1_455 ?
O6 Si3 Ce3 88.5(4) . 1_455 ?
O5 Si3 Ce3 169.5(4) . 1_455 ?
Ce2 Si3 Ce3 43.75(5) 1_455 1_455 ?
Ca Si3 Ce3 145.99(11) . 1_455 ?
Ce4 Si3 Ce3 49.68(5) 1_545 1_455 ?
Ce4 Si3 Ce3 49.68(5) . 1_455 ?
O14 Si4 O14 104.3(6) 1_565 4_565 ?
O14 Si4 O15 123.2(6) 1_565 . ?
O14 Si4 O15 100.3(6) 4_565 . ?
O14 Si4 O15 100.3(6) 1_565 4_575 ?
O14 Si4 O15 123.2(6) 4_565 4_575 ?
O15 Si4 O15 26.9(11) . 4_575 ?
O14 Si4 O12 112.3(4) 1_565 . ?
O14 Si4 O12 112.3(4) 4_565 . ?
O15 Si4 O12 103.9(7) . . ?
O15 Si4 O12 103.9(7) 4_575 . ?
O14 Si4 Ce3 127.6(3) 1_565 3_665 ?
O14 Si4 Ce3 127.6(3) 4_565 3_665 ?
O15 Si4 Ce3 48.1(6) . 3_665 ?
O15 Si4 Ce3 48.1(6) 4_575 3_665 ?
O12 Si4 Ce3 57.7(4) . 3_665 ?
O14 Si4 Ce4 52.8(3) 1_565 1_655 ?
O14 Si4 Ce4 52.8(3) 4_565 1_655 ?
O15 Si4 Ce4 117.0(6) . 1_655 ?
O15 Si4 Ce4 117.0(6) 4_575 1_655 ?
O12 Si4 Ce4 137.9(4) . 1_655 ?
Ce3 Si4 Ce4 164.44(15) 3_665 1_655 ?
O14 Si4 Ce3 42.5(3) 1_565 1_565 ?
O14 Si4 Ce3 123.7(3) 4_565 1_565 ?
O15 Si4 Ce3 81.3(5) . 1_565 ?
O15 Si4 Ce3 57.9(6) 4_575 1_565 ?
O12 Si4 Ce3 121.91(12) . 1_565 ?
Ce3 Si4 Ce3 95.21(9) 3_665 1_565 ?
Ce4 Si4 Ce3 76.12(8) 1_655 1_565 ?
O14 Si4 Ce3 123.7(3) 1_565 . ?
O14 Si4 Ce3 42.5(3) 4_565 . ?
O15 Si4 Ce3 57.9(6) . . ?
O15 Si4 Ce3 81.3(5) 4_575 . ?
O12 Si4 Ce3 121.91(12) . . ?
Ce3 Si4 Ce3 95.21(9) 3_665 . ?
Ce4 Si4 Ce3 76.12(8) 1_655 . ?
Ce3 Si4 Ce3 109.76(12) 1_565 . ?
O14 Si4 Ce2 27.1(3) 1_565 1_565 ?
O14 Si4 Ce2 107.7(3) 4_565 1_565 ?
O15 Si4 Ce2 143.5(5) . 1_565 ?
O15 Si4 Ce2 116.9(5) 4_575 1_565 ?
O12 Si4 Ce2 86.8(2) . 1_565 ?
Ce3 Si4 Ce2 121.44(7) 3_665 1_565 ?
Ce4 Si4 Ce2 66.65(7) 1_655 1_565 ?
Ce3 Si4 Ce2 63.86(3) 1_565 1_565 ?
Ce3 Si4 Ce2 142.72(13) . 1_565 ?
O14 Si4 Ce2 107.7(3) 1_565 . ?
O14 Si4 Ce2 27.1(3) 4_565 . ?
O15 Si4 Ce2 116.9(5) . . ?
O15 Si4 Ce2 143.5(5) 4_575 . ?
O12 Si4 Ce2 86.8(2) . . ?
Ce3 Si4 Ce2 121.44(7) 3_665 . ?
Ce4 Si4 Ce2 66.66(7) 1_655 . ?
Ce3 Si4 Ce2 142.72(13) 1_565 . ?
Ce3 Si4 Ce2 63.87(3) . . ?
Ce2 Si4 Ce2 98.17(10) 1_565 . ?
O17 Si5 O16 110.5(7) . . ?
O17 Si5 O13 108.6(4) . . ?
O16 Si5 O13 108.6(4) . . ?
O17 Si5 O13 108.6(4) . 4_565 ?
O16 Si5 O13 108.6(4) . 4_565 ?
O13 Si5 O13 112.1(5) . 4_565 ?
O17 Si5 Ce3 41.2(5) . 1_455 ?
O16 Si5 Ce3 69.3(6) . 1_455 ?
O13 Si5 Ce3 122.8(3) . 1_455 ?
O13 Si5 Ce3 122.8(3) 4_565 1_455 ?
O17 Si5 Ce4 58.76(13) . . ?
O16 Si5 Ce4 112.9(3) . . ?
O13 Si5 Ce4 51.6(3) . . ?
O13 Si5 Ce4 138.5(3) 4_565 . ?
Ce3 Si5 Ce4 75.83(7) 1_455 . ?
O17 Si5 Ce4 58.76(13) . 1_545 ?
O16 Si5 Ce4 112.9(3) . 1_545 ?
O13 Si5 Ce4 138.5(3) . 1_545 ?
O13 Si5 Ce4 51.6(3) 4_565 1_545 ?
Ce3 Si5 Ce4 75.83(7) 1_455 1_545 ?
Ce4 Si5 Ce4 111.35(12) . 1_545 ?
O17 Si5 Ce3 124.74(12) . 3_655 ?
O16 Si5 Ce3 68.1(3) . 3_655 ?
O13 Si5 Ce3 124.6(3) . 3_655 ?
O13 Si5 Ce3 40.5(3) 4_565 3_655 ?
Ce3 Si5 Ce3 107.86(8) 1_455 3_655 ?
Ce4 Si5 Ce3 176.14(12) . 3_655 ?
Ce4 Si5 Ce3 71.07(2) 1_545 3_655 ?
O17 Si5 Ce3 124.74(12) . 3_665 ?
O16 Si5 Ce3 68.1(3) . 3_665 ?
O13 Si5 Ce3 40.5(3) . 3_665 ?
O13 Si5 Ce3 124.6(3) 4_565 3_665 ?
Ce3 Si5 Ce3 107.86(8) 1_455 3_665 ?
Ce4 Si5 Ce3 71.07(2) . 3_665 ?
Ce4 Si5 Ce3 176.14(12) 1_545 3_665 ?
Ce3 Si5 Ce3 106.35(11) 3_655 3_665 ?
O17 Si5 Ce4 109.5(5) . 3_565 ?
O16 Si5 Ce4 1.0(6) . 3_565 ?
O13 Si5 Ce4 109.0(3) . 3_565 ?
O13 Si5 Ce4 109.0(3) 4_565 3_565 ?
Ce3 Si5 Ce4 68.29(7) 1_455 3_565 ?
Ce4 Si5 Ce4 112.42(7) . 3_565 ?
Ce4 Si5 Ce4 112.42(7) 1_545 3_565 ?
Ce3 Si5 Ce4 68.60(7) 3_655 3_565 ?
Ce3 Si5 Ce4 68.60(7) 3_665 3_565 ?
O17 Si5 Ce2 14.2(4) . 1_455 ?
O16 Si5 Ce2 124.7(6) . 1_455 ?
O13 Si5 Ce2 101.3(3) . 1_455 ?
O13 Si5 Ce2 101.3(3) 4_565 1_455 ?
Ce3 Si5 Ce2 55.39(6) 1_455 1_455 ?
Ce4 Si5 Ce2 56.15(6) . 1_455 ?
Ce4 Si5 Ce2 56.15(6) 1_545 1_455 ?
Ce3 Si5 Ce2 126.73(5) 3_655 1_455 ?
Ce3 Si5 Ce2 126.73(5) 3_665 1_455 ?
Ce4 Si5 Ce2 123.68(9) 3_565 1_455 ?
Si1 O1 Fe1 124.3(4) . . ?
Si1 O1 Fe3 124.1(4) . . ?
Fe1 O1 Fe3 90.4(3) . . ?
Si1 O1 Ce 112.1(4) . 3_666 ?
Fe1 O1 Ce 102.1(3) . 3_666 ?
Fe3 O1 Ce 98.7(3) . 3_666 ?
Si1 O1 Ce2 59.6(3) . 1_455 ?
Fe1 O1 Ce2 118.6(3) . 1_455 ?
Fe3 O1 Ce2 65.54(19) . 1_455 ?
Ce O1 Ce2 135.4(3) 3_666 1_455 ?
Si1 O1 Ce 40.4(2) . 1_455 ?
Fe1 O1 Ce 162.0(3) . 1_455 ?
Fe3 O1 Ce 94.2(2) . 1_455 ?
Ce O1 Ce 94.4(2) 3_666 1_455 ?
Ce2 O1 Ce 49.14(9) 1_455 1_455 ?
Si1 O1 Ce 32.6(2) . 3_656 ?
Fe1 O1 Ce 98.1(3) . 3_656 ?
Fe3 O1 Ce 152.9(3) . 3_656 ?
Ce O1 Ce 104.5(3) 3_666 3_656 ?
Ce2 O1 Ce 87.92(14) 1_455 3_656 ?
Ce O1 Ce 70.51(12) 1_455 3_656 ?
Si3 O2 Fe3 126.4(4) . . ?
Si3 O2 Ce4 130.0(4) . . ?
Fe3 O2 Ce4 92.6(3) . . ?
Si3 O2 Ce2 99.3(4) . 1_455 ?
Fe3 O2 Ce2 105.7(3) . 1_455 ?
Ce4 O2 Ce2 98.0(2) . 1_455 ?
Si3 O2 Ce4 51.1(3) . 1_545 ?
Fe3 O2 Ce4 158.7(3) . 1_545 ?
Ce4 O2 Ce4 103.3(2) . 1_545 ?
Ce2 O2 Ce4 58.52(15) 1_455 1_545 ?
Si3 O2 Ce3 101.1(3) . 1_455 ?
Fe3 O2 Ce3 131.4(3) . 1_455 ?
Ce4 O2 Ce3 57.98(15) . 1_455 ?
Ce2 O2 Ce3 50.60(13) 1_455 1_455 ?
Ce4 O2 Ce3 52.09(8) 1_545 1_455 ?
Si3 O2 Ce2 169.5(4) . 1_465 ?
Fe3 O2 Ce2 46.84(16) . 1_465 ?
Ce4 O2 Ce2 50.31(14) . 1_465 ?
Ce2 O2 Ce2 90.83(17) 1_455 1_465 ?
Ce4 O2 Ce2 138.69(16) 1_545 1_465 ?
Ce3 O2 Ce2 87.53(11) 1_455 1_465 ?
Si2 O3 Fe2 124.9(5) . 1_565 ?
Si2 O3 Ce 111.9(4) . 1_565 ?
Fe2 O3 Ce 115.2(4) 1_565 1_565 ?
Si2 O3 Ce2 102.2(3) . 1_565 ?
Fe2 O3 Ce2 103.7(3) 1_565 1_565 ?
Ce O3 Ce2 91.4(3) 1_565 1_565 ?
Si2 O3 Ce2 29.4(2) . . ?
Fe2 O3 Ce2 100.7(3) 1_565 . ?
Ce O3 Ce2 141.1(3) 1_565 . ?
Ce2 O3 Ce2 94.37(18) 1_565 . ?
Si2 O3 Ce4 107.4(3) . . ?
Fe2 O3 Ce4 31.80(19) 1_565 . ?
Ce O3 Ce4 107.0(2) 1_565 . ?
Ce2 O3 Ce4 135.5(2) 1_565 . ?
Ce2 O3 Ce4 95.43(13) . . ?
Fe1 O4 Fe1 99.6(5) 2_656 . ?
Fe1 O4 Fe3 102.8(4) 2_656 . ?
Fe1 O4 Fe3 102.8(4) . . ?
Fe1 O4 Ce 62.8(3) 2_656 3_666 ?
Fe1 O4 Ce 62.8(3) . 3_666 ?
Fe3 O4 Ce 65.2(3) . 3_666 ?
Fe1 O4 Ce 60.0(2) 2_656 1_565 ?
Fe1 O4 Ce 127.1(4) . 1_565 ?
Fe3 O4 Ce 128.2(2) . 1_565 ?
Ce O4 Ce 122.83(19) 3_666 1_565 ?
Fe1 O4 Ce4 127.7(3) 2_656 . ?
Fe1 O4 Ce4 127.7(3) . . ?
Fe3 O4 Ce4 51.5(3) . . ?
Ce O4 Ce4 116.7(3) 3_666 . ?
Ce O4 Ce4 98.1(2) 1_565 . ?
Si3 O5 Fe1 128.6(3) . . ?
Si3 O5 Fe1 128.6(3) . 2_646 ?
Fe1 O5 Fe1 90.0(4) . 2_646 ?
Si3 O5 Ca 108.2(5) . . ?
Fe1 O5 Ca 97.0(3) . . ?
Fe1 O5 Ca 97.0(3) 2_646 . ?
Si3 O5 Ce2 36.9(3) . 1_455 ?
Fe1 O5 Ce2 107.4(3) . 1_455 ?
Fe1 O5 Ce2 107.4(3) 2_646 1_455 ?
Ca O5 Ce2 145.1(4) . 1_455 ?
Si3 O5 Ce4 34.69(6) . 1_545 ?
Fe1 O5 Ce4 155.4(4) . 1_545 ?
Fe1 O5 Ce4 96.04(16) 2_646 1_545 ?
Ca O5 Ce4 105.8(3) . 1_545 ?
Ce2 O5 Ce4 48.14(9) 1_455 1_545 ?
Si3 O5 Ce4 34.69(6) . . ?
Fe1 O5 Ce4 96.04(16) . . ?
Fe1 O5 Ce4 155.4(4) 2_646 . ?
Ca O5 Ce4 105.8(3) . . ?
Ce2 O5 Ce4 48.14(9) 1_455 . ?
Ce4 O5 Ce4 69.35(13) 1_545 . ?
Si3 O5 Ce 110.1(4) . 3_666 ?
Fe1 O5 Ce 30.0(2) . 3_666 ?
Fe1 O5 Ce 86.4(3) 2_646 3_666 ?
Ca O5 Ce 127.1(2) . 3_666 ?
Ce2 O5 Ce 79.97(15) 1_455 3_666 ?
Ce4 O5 Ce 126.4(2) 1_545 3_666 ?
Ce4 O5 Ce 86.97(10) . 3_666 ?
Si3 O5 Ce 110.1(4) . 3_656 ?
Fe1 O5 Ce 86.4(3) . 3_656 ?
Fe1 O5 Ce 30.0(2) 2_646 3_656 ?
Ca O5 Ce 127.1(2) . 3_656 ?
Ce2 O5 Ce 79.97(15) 1_455 3_656 ?
Ce4 O5 Ce 86.97(10) 1_545 3_656 ?
Ce4 O5 Ce 126.4(2) . 3_656 ?
Ce O5 Ce 69.27(15) 3_666 3_656 ?
Si3 O6 Fe2 131.8(3) . 4_565 ?
Si3 O6 Fe2 131.8(3) . . ?
Fe2 O6 Fe2 95.1(5) 4_565 . ?
Si3 O6 Ca 94.1(4) . . ?
Fe2 O6 Ca 93.6(3) 4_565 . ?
Fe2 O6 Ca 93.6(3) . . ?
Si3 O6 Ce4 72.1(3) . 1_545 ?
Fe2 O6 Ce4 132.1(4) 4_565 1_545 ?
Fe2 O6 Ce4 66.57(19) . 1_545 ?
Ca O6 Ce4 129.60(15) . 1_545 ?
Si3 O6 Ce4 72.1(3) . . ?
Fe2 O6 Ce4 66.56(19) 4_565 . ?
Fe2 O6 Ce4 132.1(4) . . ?
Ca O6 Ce4 129.60(15) . . ?
Ce4 O6 Ce4 92.8(2) 1_545 . ?
Si3 O6 Ce2 150.8(5) . . ?
Fe2 O6 Ce2 58.2(3) 4_565 . ?
Fe2 O6 Ce2 58.2(3) . . ?
Ca O6 Ce2 56.70(17) . . ?
Ce4 O6 Ce2 124.71(16) 1_545 . ?
Ce4 O6 Ce2 124.71(16) . . ?
Si3 O6 Ce2 32.4(3) . 1_455 ?
Fe2 O6 Ce2 120.2(3) 4_565 1_455 ?
Fe2 O6 Ce2 120.2(3) . 1_455 ?
Ca O6 Ce2 126.5(3) . 1_455 ?
Ce4 O6 Ce2 53.83(12) 1_545 1_455 ?
Ce4 O6 Ce2 53.83(12) . 1_455 ?
Ce2 O6 Ce2 176.8(3) . 1_455 ?
Si1 O7 Ce2 136.1(6) . 1_455 ?
Si1 O7 Ce 121.9(6) . 1_455 ?
Ce2 O7 Ce 102.0(4) 1_455 1_455 ?
Si1 O7 Ce 44.22(14) . 3_666 ?
Ce2 O7 Ce 132.03(19) 1_455 3_666 ?
Ce O7 Ce 101.0(3) 1_455 3_666 ?
Si1 O7 Ce 44.22(14) . 3_656 ?
Ce2 O7 Ce 132.03(19) 1_455 3_656 ?
Ce O7 Ce 101.0(3) 1_455 3_656 ?
Ce O7 Ce 82.84(18) 3_666 3_656 ?
Si2 O8 Fe3 129.3(7) . 1_655 ?
Si2 O8 Ce2 93.3(2) . . ?
Fe3 O8 Ce2 100.9(2) 1_655 . ?
Si2 O8 Ce2 93.3(2) . 1_565 ?
Fe3 O8 Ce2 100.9(2) 1_655 1_565 ?
Ce2 O8 Ce2 145.3(4) . 1_565 ?
Si2 O8 Ce4 151.2(6) . 1_655 ?
Fe3 O8 Ce4 79.5(3) 1_655 1_655 ?
Ce2 O8 Ce4 79.0(2) . 1_655 ?
Ce2 O8 Ce4 79.0(2) 1_565 1_655 ?
Si2 O8 Ce 43.87(14) . 1_565 ?
Fe3 O8 Ce 108.3(3) 1_655 1_565 ?
Ce2 O8 Ce 137.2(3) . 1_565 ?
Ce2 O8 Ce 57.21(12) 1_565 1_565 ?
Ce4 O8 Ce 136.14(15) 1_655 1_565 ?
Si2 O8 Ce 82.3(5) . 3_766 ?
Fe3 O8 Ce 47.0(3) 1_655 3_766 ?
Ce2 O8 Ce 107.3(2) . 3_766 ?
Ce2 O8 Ce 107.3(2) 1_565 3_766 ?
Ce4 O8 Ce 126.5(3) 1_655 3_766 ?
Ce O8 Ce 73.75(18) 1_565 3_766 ?
Si2 O9 Si1 148.2(8) . 3_666 ?
Si2 O9 Ce 83.2(3) . 1_565 ?
Si1 O9 Ce 85.0(3) 3_666 1_565 ?
Si2 O9 Ca 83.2(3) . . ?
Si1 O9 Ca 85.0(3) 3_666 . ?
Ce O9 Ca 135.6(4) 1_565 . ?
Si2 O9 Ce 132.1(6) . 3_766 ?
Si1 O9 Ce 79.6(4) 3_666 3_766 ?
Ce O9 Ce 110.2(2) 1_565 3_766 ?
Ca O9 Ce 110.2(2) . 3_766 ?
Si2 O9 Ce2 46.01(18) . . ?
Si1 O9 Ce2 138.96(14) 3_666 . ?
Ce O9 Ce2 129.0(3) 1_565 . ?
Ca O9 Ce2 55.15(12) . . ?
Ce O9 Ce2 103.6(2) 3_766 . ?
Si2 O9 Ce2 46.01(18) . 1_565 ?
Si1 O9 Ce2 138.96(14) 3_666 1_565 ?
Ce O9 Ce2 55.15(12) 1_565 1_565 ?
Ca O9 Ce2 129.0(3) . 1_565 ?
Ce O9 Ce2 103.6(2) 3_766 1_565 ?
Ce2 O9 Ce2 80.89(19) . 1_565 ?
Si2 O9 Ce2 179.7(6) . 3_766 ?
Si1 O9 Ce2 32.0(3) 3_666 3_766 ?
Ce O9 Ce2 96.9(2) 1_565 3_766 ?
Ca O9 Ce2 96.9(2) . 3_766 ?
Ce O9 Ce2 47.60(14) 3_766 3_766 ?
Ce2 O9 Ce2 133.88(15) . 3_766 ?
Ce2 O9 Ce2 133.88(15) 1_565 3_766 ?
Fe2 O10 Fe2 99.2(5) . 4_565 ?
Fe2 O10 Ce2 106.8(4) . . ?
Fe2 O10 Ce2 106.8(4) 4_565 . ?
Fe2 O10 Ce3 129.9(3) . . ?
Fe2 O10 Ce3 129.9(3) 4_565 . ?
Ce2 O10 Ce3 71.8(2) . . ?
Fe2 O10 Ce3 62.5(2) . 3_655 ?
Fe2 O10 Ce3 125.6(4) 4_565 3_655 ?
Ce2 O10 Ce3 127.2(2) . 3_655 ?
Ce3 O10 Ce3 78.73(17) . 3_655 ?
Fe2 O10 Ce3 125.6(4) . 3_665 ?
Fe2 O10 Ce3 62.5(2) 4_565 3_665 ?
Ce2 O10 Ce3 127.2(2) . 3_665 ?
Ce3 O10 Ce3 78.73(17) . 3_665 ?
Ce3 O10 Ce3 86.5(2) 3_655 3_665 ?
Fe2 O10 H1 111(7) . . ?
Fe2 O10 H1 111(7) 4_565 . ?
Ce2 O10 H1 121(10) . . ?
Ce3 O10 H1 49(10) . . ?
Ce3 O10 H1 49(5) 3_655 . ?
Ce3 O10 H1 49(5) 3_665 . ?
Fe2 O11 Fe2 99.0(5) 4_565 1_565 ?
Fe2 O11 Ce4 107.5(3) 4_565 . ?
Fe2 O11 Ce4 107.5(3) 1_565 . ?
Fe2 O11 Ce3 63.6(3) 4_565 3_665 ?
Fe2 O11 Ce3 63.6(3) 1_565 3_665 ?
Ce4 O11 Ce3 70.7(2) . 3_665 ?
Fe2 O11 Ce 120.8(4) 4_565 1_565 ?
Fe2 O11 Ce 58.4(2) 1_565 1_565 ?
Ce4 O11 Ce 130.80(17) . 1_565 ?
Ce3 O11 Ce 121.88(17) 3_665 1_565 ?
Fe2 O11 H2 120(5) 4_565 . ?
Fe2 O11 H2 120(5) 1_565 . ?
Ce4 O11 H2 102(10) . . ?
Ce3 O11 H2 172(10) 3_665 . ?
Ce O11 H2 63(7) 1_565 . ?
Si4 O12 Fe2 130.3(3) . 1_565 ?
Si4 O12 Fe2 130.3(3) . 4_565 ?
Fe2 O12 Fe2 94.1(5) 1_565 4_565 ?
Si4 O12 Ce3 92.0(4) . 3_665 ?
Fe2 O12 Ce3 100.9(3) 1_565 3_665 ?
Fe2 O12 Ce3 100.9(3) 4_565 3_665 ?
Si4 O12 Ce2 68.9(2) . . ?
Fe2 O12 Ce2 128.4(4) 1_565 . ?
Fe2 O12 Ce2 65.63(19) 4_565 . ?
Ce3 O12 Ce2 128.45(18) 3_665 . ?
Si4 O12 Ce2 68.9(2) . 1_565 ?
Fe2 O12 Ce2 65.63(19) 1_565 1_565 ?
Fe2 O12 Ce2 128.4(4) 4_565 1_565 ?
Ce3 O12 Ce2 128.45(18) 3_665 1_565 ?
Ce2 O12 Ce2 89.82(18) . 1_565 ?
Si4 O12 Ce4 159.0(5) . . ?
Fe2 O12 Ce4 58.1(3) 1_565 . ?
Fe2 O12 Ce4 58.1(3) 4_565 . ?
Ce3 O12 Ce4 66.97(19) 3_665 . ?
Ce2 O12 Ce4 123.73(17) . . ?
Ce2 O12 Ce4 123.73(17) 1_565 . ?
Si4 O12 Ce3 40.15(12) . 1_565 ?
Fe2 O12 Ce3 94.40(17) 1_565 1_565 ?
Fe2 O12 Ce3 170.5(3) 4_565 1_565 ?
Ce3 O12 Ce3 81.6(2) 3_665 1_565 ?
Ce2 O12 Ce3 105.6(2) . 1_565 ?
Ce2 O12 Ce3 52.48(8) 1_565 1_565 ?
Ce4 O12 Ce3 130.66(15) . 1_565 ?
Si4 O12 Ce3 40.14(12) . . ?
Fe2 O12 Ce3 170.5(3) 1_565 . ?
Fe2 O12 Ce3 94.40(17) 4_565 . ?
Ce3 O12 Ce3 81.6(2) 3_665 . ?
Ce2 O12 Ce3 52.49(8) . . ?
Ce2 O12 Ce3 105.6(2) 1_565 . ?
Ce4 O12 Ce3 130.66(15) . . ?
Ce3 O12 Ce3 76.81(16) 1_565 . ?
Si4 O12 Ce4 28.3(3) . 1_655 ?
Fe2 O12 Ce4 118.0(3) 1_565 1_655 ?
Fe2 O12 Ce4 118.0(3) 4_565 1_655 ?
Ce3 O12 Ce4 120.3(3) 3_665 1_655 ?
Ce2 O12 Ce4 52.67(11) . 1_655 ?
Ce2 O12 Ce4 52.67(11) 1_565 1_655 ?
Ce4 O12 Ce4 172.7(3) . 1_655 ?
Ce3 O12 Ce4 53.75(11) 1_565 1_655 ?
Ce3 O12 Ce4 53.75(11) . 1_655 ?
Si4 O12 Ce 113.6(3) . 1_565 ?
Fe2 O12 Ce 34.2(2) 1_565 1_565 ?
Fe2 O12 Ce 90.2(3) 4_565 1_565 ?
Ce3 O12 Ce 134.83(18) 3_665 1_565 ?
Ce2 O12 Ce 96.11(19) . 1_565 ?
Ce2 O12 Ce 45.96(9) 1_565 1_565 ?
Ce4 O12 Ce 83.38(16) . 1_565 ?
Ce3 O12 Ce 94.43(8) 1_565 1_565 ?
Ce3 O12 Ce 141.5(2) . 1_565 ?
Ce4 O12 Ce 90.65(15) 1_655 1_565 ?
Si5 O13 Fe2 123.6(5) . 4_565 ?
Si5 O13 Ce3 114.9(4) . 3_665 ?
Fe2 O13 Ce3 111.2(3) 4_565 3_665 ?
Si5 O13 Ce4 100.7(3) . . ?
Fe2 O13 Ce4 100.9(3) 4_565 . ?
Ce3 O13 Ce4 100.4(2) 3_665 . ?
Si5 O13 Ce3 39.3(2) . 1_455 ?
Fe2 O13 Ce3 145.8(3) 4_565 1_455 ?
Ce3 O13 Ce3 102.4(2) 3_665 1_455 ?
Ce4 O13 Ce3 66.08(14) . 1_455 ?
Si5 O13 Ce4 51.6(3) . 3_565 ?
Fe2 O13 Ce4 151.5(3) 4_565 3_565 ?
Ce3 O13 Ce4 63.39(15) 3_665 3_565 ?
Ce4 O13 Ce4 107.53(19) . 3_565 ?
Ce3 O13 Ce4 53.03(8) 1_455 3_565 ?
Si5 O13 Ce3 38.7(2) . 3_655 ?
Fe2 O13 Ce3 103.9(3) 4_565 3_655 ?
Ce3 O13 Ce3 99.8(2) 3_665 3_655 ?
Ce4 O13 Ce3 139.4(2) . 3_655 ?
Ce3 O13 Ce3 75.41(11) 1_455 3_655 ?
Ce4 O13 Ce3 53.29(8) 3_565 3_655 ?
Si5 O13 Ce4 28.5(2) . 1_545 ?
Fe2 O13 Ce4 98.7(3) 4_565 1_545 ?
Ce3 O13 Ce4 143.2(2) 3_665 1_545 ?
Ce4 O13 Ce4 94.13(19) . 1_545 ?
Ce3 O13 Ce4 53.63(8) 1_455 1_545 ?
Ce4 O13 Ce4 80.04(11) 3_565 1_545 ?
Ce3 O13 Ce4 50.90(8) 3_655 1_545 ?
Si4 O14 Ce2 135.5(4) 1_545 . ?
Si4 O14 Ce3 112.2(4) 1_545 . ?
Ce2 O14 Ce3 100.7(3) . . ?
Si4 O14 Ce4 98.4(4) 1_545 1_645 ?
Ce2 O14 Ce4 99.6(3) . 1_645 ?
Ce3 O14 Ce4 107.1(3) . 1_645 ?
Si4 O14 Ce3 35.8(2) 1_545 3_655 ?
Ce2 O14 Ce3 123.7(2) . 3_655 ?
Ce3 O14 Ce3 86.7(2) . 3_655 ?
Ce4 O14 Ce3 131.6(3) 1_645 3_655 ?
Si4 O14 Ce2 52.5(3) 1_545 1_545 ?
Ce2 O14 Ce2 105.7(2) . 1_545 ?
Ce3 O14 Ce2 152.0(3) . 1_545 ?
Ce4 O14 Ce2 59.30(15) 1_645 1_545 ?
Ce3 O14 Ce2 86.66(14) 3_655 1_545 ?
Si4 O14 Ce3 39.3(2) 1_545 1_545 ?
Ce2 O14 Ce3 154.9(3) . 1_545 ?
Ce3 O14 Ce3 102.6(2) . 1_545 ?
Ce4 O14 Ce3 64.51(16) 1_645 1_545 ?
Ce3 O14 Ce3 67.28(12) 3_655 1_545 ?
Ce2 O14 Ce3 49.97(9) 1_545 1_545 ?
Si4 O14 Ce4 167.6(4) 1_545 1_655 ?
Ce2 O14 Ce4 49.85(14) . 1_655 ?
Ce3 O14 Ce4 56.61(15) . 1_655 ?
Ce4 O14 Ce4 90.64(19) 1_645 1_655 ?
Ce3 O14 Ce4 132.60(18) 3_655 1_655 ?
Ce2 O14 Ce4 139.84(19) 1_545 1_655 ?
Ce3 O14 Ce4 142.70(16) 1_545 1_655 ?
O15 O15 Si4 76.6(5) 4_575 . ?
O15 O15 Ce3 81.4(3) 4_575 3_665 ?
Si4 O15 Ce3 103.2(7) . 3_665 ?
O15 O15 Ce3 146.6(3) 4_575 . ?
Si4 O15 Ce3 94.4(6) . . ?
Ce3 O15 Ce3 131.9(6) 3_665 . ?
O15 O15 Ce3 26.8(3) 4_575 1_565 ?
Si4 O15 Ce3 72.3(5) . 1_565 ?
Ce3 O15 Ce3 108.1(5) 3_665 1_565 ?
Ce3 O15 Ce3 119.8(5) . 1_565 ?
O15 O15 Ce4 85.0(2) 4_575 1_655 ?
Si4 O15 Ce4 43.3(5) . 1_655 ?
Ce3 O15 Ce4 146.2(5) 3_665 1_655 ?
Ce3 O15 Ce4 67.7(3) . 1_655 ?
Ce3 O15 Ce4 63.3(2) 1_565 1_655 ?
O15 O15 Ce2 85.21(19) 4_575 3_665 ?
Si4 O15 Ce2 156.1(7) . 3_665 ?
Ce3 O15 Ce2 58.2(3) 3_665 3_665 ?
Ce3 O15 Ce2 109.2(4) . 3_665 ?
Ce3 O15 Ce2 97.9(3) 1_565 3_665 ?
Ce4 O15 Ce2 150.8(4) 1_655 3_665 ?
O15 O15 Ce2 121.49(18) 4_575 . ?
Si4 O15 Ce2 45.3(4) . . ?
Ce3 O15 Ce2 112.9(4) 3_665 . ?
Ce3 O15 Ce2 54.2(2) . . ?
Ce3 O15 Ce2 110.2(3) 1_565 . ?
Ce4 O15 Ce2 51.02(16) 1_655 . ?
Ce2 O15 Ce2 151.8(4) 3_665 . ?
Si5 O16 Ce4 178.3(9) . 3_565 ?
Si5 O16 Ce3 82.9(6) . 1_455 ?
Ce4 O16 Ce3 95.4(5) 3_565 1_455 ?
Si5 O16 Ce3 85.7(3) . 3_665 ?
Ce4 O16 Ce3 95.2(3) 3_565 3_665 ?
Ce3 O16 Ce3 119.4(2) 1_455 3_665 ?
Si5 O16 Ce3 85.7(3) . 3_655 ?
Ce4 O16 Ce3 95.2(3) 3_565 3_655 ?
Ce3 O16 Ce3 119.4(2) 1_455 3_655 ?
Ce3 O16 Ce3 118.7(4) 3_665 3_655 ?
Si5 O16 Ce4 47.4(2) . . ?
Ce4 O16 Ce4 131.8(3) 3_565 . ?
Ce3 O16 Ce4 66.0(2) 1_455 . ?
Ce3 O16 Ce4 62.96(11) 3_665 . ?
Ce3 O16 Ce4 132.9(3) 3_655 . ?
Si5 O16 Ce4 47.4(2) . 1_545 ?
Ce4 O16 Ce4 131.8(3) 3_565 1_545 ?
Ce3 O16 Ce4 66.0(2) 1_455 1_545 ?
Ce3 O16 Ce4 132.9(3) 3_665 1_545 ?
Ce3 O16 Ce4 62.96(11) 3_655 1_545 ?
Ce4 O16 Ce4 82.6(2) . 1_545 ?
Si5 O16 Ce2 134.1(4) . 3_655 ?
Ce4 O16 Ce2 47.0(2) 3_565 3_655 ?
Ce3 O16 Ce2 122.1(3) 1_455 3_655 ?
Ce3 O16 Ce2 107.9(3) 3_665 3_655 ?
Ce3 O16 Ce2 49.05(15) 3_655 3_655 ?
Ce4 O16 Ce2 170.8(3) . 3_655 ?
Ce4 O16 Ce2 104.37(4) 1_545 3_655 ?
Si5 O16 Ce2 134.1(4) . 3_665 ?
Ce4 O16 Ce2 47.0(2) 3_565 3_665 ?
Ce3 O16 Ce2 122.1(3) 1_455 3_665 ?
Ce3 O16 Ce2 49.05(15) 3_665 3_665 ?
Ce3 O16 Ce2 107.9(3) 3_655 3_665 ?
Ce4 O16 Ce2 104.37(4) . 3_665 ?
Ce4 O16 Ce2 170.8(3) 1_545 3_665 ?
Ce2 O16 Ce2 68.08(17) 3_655 3_665 ?
Si5 O17 Ce3 113.3(7) . 1_455 ?
Si5 O17 Ce4 94.1(2) . . ?
Ce3 O17 Ce4 102.1(2) 1_455 . ?
Si5 O17 Ce4 94.1(2) . 1_545 ?
Ce3 O17 Ce4 102.1(2) 1_455 1_545 ?
Ce4 O17 Ce4 148.9(5) . 1_545 ?
Si5 O17 Ce2 158.5(7) . 1_455 ?
Ce3 O17 Ce2 88.2(3) 1_455 1_455 ?
Ce4 O17 Ce2 80.7(2) . 1_455 ?
Ce4 O17 Ce2 80.7(2) 1_545 1_455 ?
Si5 O17 Ce4 51.8(4) . 3_565 ?
Ce3 O17 Ce4 61.5(3) 1_455 3_565 ?
Ce4 O17 Ce4 104.3(2) . 3_565 ?
Ce4 O17 Ce4 104.3(2) 1_545 3_565 ?
Ce2 O17 Ce4 149.7(3) 1_455 3_565 ?
Si5 O17 Ce3 39.04(13) . 3_665 ?
Ce3 O17 Ce3 100.2(3) 1_455 3_665 ?
Ce4 O17 Ce3 60.06(14) . 3_665 ?
Ce4 O17 Ce3 133.1(3) 1_545 3_665 ?
Ce2 O17 Ce3 140.80(13) 1_455 3_665 ?
Ce4 O17 Ce3 53.68(13) 3_565 3_665 ?
Si5 O17 Ce3 39.04(13) . 3_655 ?
Ce3 O17 Ce3 100.2(3) 1_455 3_655 ?
Ce4 O17 Ce3 133.1(3) . 3_655 ?
Ce4 O17 Ce3 60.06(14) 1_545 3_655 ?
Ce2 O17 Ce3 140.80(13) 1_455 3_655 ?
Ce4 O17 Ce3 53.68(13) 3_565 3_655 ?
Ce3 O17 Ce3 75.69(19) 3_665 3_655 ?
 
loop_
 _geom_hbond_atom_site_label_D 
 _geom_hbond_atom_site_label_H 
 _geom_hbond_atom_site_label_A 
 _geom_hbond_distance_DH 
 _geom_hbond_distance_HA 
 _geom_hbond_distance_DA 
 _geom_hbond_angle_DHA 
 _geom_hbond_site_symmetry_A 
 _geom_hbond_publ_flag
O10 H1 O15  0.850(10) 1.91(3) 2.735(18) 165(10) 3_665 yes
O10 H1 O15  0.850(10) 1.91(3) 2.735(18) 165(10) 2_645 yes
O11 H2 O4  0.851(10) 2.14(2) 2.992(15) 177(15) . yes
 
_refine_diff_density_max    2.347
_refine_diff_density_min   -2.136
_refine_diff_density_rms    0.326



